# Supplementary Information (SI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_m9173_0m_a
_database_code_depnum_ccdc_archive 'CCDC 2326212'
loop_
_audit_author_name
_audit_author_address
chen
;henan univwersity
China
;
_audit_update_record             
;
2024-01-17 deposited with the CCDC.	2024-08-23 downloaded from the CCDC.
;
_audit_creation_date             2022-10-05
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'K Na11 O127 Si2 Ta24, 31.5(O)'
_chemical_formula_sum            'K Na11 O158.50 Si2 Ta24'
_chemical_formula_weight         7226.97
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   19.495(5)
_cell_length_b                   19.844(6)
_cell_length_c                   21.896(7)
_cell_angle_alpha                73.755(10)
_cell_angle_beta                 81.216(7)
_cell_angle_gamma                66.588(8)
_cell_volume                     7455(4)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9246
_cell_measurement_temperature    150
_cell_measurement_theta_max      28.288
_cell_measurement_theta_min      2.280
_shelx_estimated_absorpt_T_max   0.270
_shelx_estimated_absorpt_T_min   0.225
_exptl_absorpt_coefficient_mu    17.730
_exptl_absorpt_correction_T_max  0.0962
_exptl_absorpt_correction_T_min  0.0393
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1722 before and 0.0833 after correction. The Ratio of minimum to maximum transmission is 0.4085. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.219
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             6376
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.1
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0828
_diffrn_reflns_av_unetI/netI     0.0539
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            155083
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.100
_diffrn_reflns_theta_max         25.100
_diffrn_reflns_theta_min         1.900
_diffrn_ambient_temperature      150.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker D8 VENTURE PHOTON II'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  'Helios multilayer optic'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_source_source            'Incoatc Ius 3.0 '
_diffrn_source_type              Microfocus
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                21870
_reflns_number_total             26519
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         4.050
_refine_diff_density_min         -3.023
_refine_diff_density_rms         0.356
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1736
_refine_ls_number_reflns         26519
_refine_ls_number_restraints     60
_refine_ls_R_factor_all          0.0560
_refine_ls_R_factor_gt           0.0437
_refine_ls_restrained_S_all      1.023
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0629P)²+148.2298P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1111
_refine_ls_wR_factor_ref         0.1222
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O37W) \\sim Ueq, Uanis(O42W) \\sim Ueq, Uanis(Na10) \\sim Ueq,
Uanis(Na11) \\sim Ueq, Uanis(O49W) \\sim Ueq, Uanis(O50W) \\sim Ueq,
Uanis(O53W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O45W) \\sim Ueq, Uanis(O47W) \\sim Ueq, Uanis(O54W) \\sim Ueq: with sigma
of 0.005 and sigma for terminal atoms of 0.01
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.77078(3) 0.18316(3) 0.78113(3) 0.02660(13) Uani 1 1 d . . . . .
Ta2 Ta 0.64413(3) 0.10853(3) 0.79149(3) 0.02410(13) Uani 1 1 d . . . . .
Ta3 Ta 0.63450(3) 0.22069(3) 0.88874(3) 0.02299(12) Uani 1 1 d . . . . .
Ta4 Ta 0.60842(3) 0.27540(3) 0.69663(3) 0.02299(12) Uani 1 1 d . . . . .
Ta5 Ta 0.46139(3) 0.24904(3) 0.81763(3) 0.02083(12) Uani 1 1 d . . . . .
Ta6 Ta 0.29543(3) 0.25365(3) 0.75085(3) 0.02158(12) Uani 1 1 d . . . . .
Ta7 Ta 0.31297(3) 0.19838(3) 0.91387(3) 0.02198(12) Uani 1 1 d . . . . .
Ta8 Ta 0.15225(3) 0.31204(3) 0.84798(3) 0.02305(13) Uani 1 1 d . . . . .
Ta9 Ta 0.28246(3) 0.37802(3) 0.87530(2) 0.01904(12) Uani 1 1 d . . . . .
Ta10 Ta 0.18694(3) 0.45931(3) 0.72442(3) 0.02102(12) Uani 1 1 d . . . . .
Ta11 Ta 0.08465(3) 0.56622(3) 0.58186(3) 0.02016(12) Uani 1 1 d . . . . .
Ta12 Ta 0.04314(3) 0.65415(3) 0.70338(2) 0.01870(12) Uani 1 1 d . . . . .
Ta13 Ta 0.23484(3) 0.59803(3) 0.58985(2) 0.01644(11) Uani 1 1 d . . . . .
Ta14 Ta 0.06340(3) 0.74515(3) 0.55662(2) 0.01876(12) Uani 1 1 d . . . . .
Ta15 Ta 0.18304(3) 0.76525(3) 0.65832(2) 0.01944(12) Uani 1 1 d . . . . .
Ta16 Ta 0.27654(3) 0.76447(3) 0.79009(2) 0.01856(12) Uani 1 1 d . . . . .
Ta17 Ta 0.13741(3) 0.92989(3) 0.71717(3) 0.02105(12) Uani 1 1 d . . . . .
Ta18 Ta 0.27534(3) 0.90252(3) 0.60981(3) 0.02033(12) Uani 1 1 d . . . . .
Ta19 Ta 0.29642(3) 0.92626(3) 0.75500(3) 0.02225(12) Uani 1 1 d . . . . .
Ta20 Ta 0.44631(3) 0.77782(3) 0.69531(3) 0.02091(12) Uani 1 1 d . . . . .
Ta21 Ta 0.62326(3) 0.79205(3) 0.62754(3) 0.02570(13) Uani 1 1 d . . . . .
Ta22 Ta 0.59487(3) 0.64929(3) 0.60864(3) 0.02359(13) Uani 1 1 d . . . . .
Ta23 Ta 0.62530(3) 0.67983(3) 0.77928(3) 0.02102(12) Uani 1 1 d . . . . .
Ta24 Ta 0.75783(3) 0.62536(3) 0.67199(3) 0.02599(13) Uani 1 1 d . . . . .
K1 K 0.3510(2) 0.5558(2) 0.41234(16) 0.0353(8) Uani 1 1 d . . . . .
Si1 Si 0.6677(2) 0.3548(2) 0.77748(18) 0.0224(8) Uani 1 1 d . . . . .
Si2 Si 0.6634(2) 0.5219(2) 0.73750(19) 0.0232(8) Uani 1 1 d . . . . .
Na1 Na 0.5091(4) 0.6491(4) 0.9807(3) 0.0387(15) Uani 1 1 d . . . . .
Na2 Na 0.5244(3) 0.8279(3) 0.8883(3) 0.0331(13) Uani 1 1 d . . . . .
Na3 Na 0.4646(3) 0.9941(3) 0.9364(3) 0.0297(12) Uani 1 1 d . . . . .
Na4 Na -0.0526(3) 0.9614(3) 0.5587(3) 0.0274(12) Uani 1 1 d . . . . .
Na5 Na 0.2248(3) 0.5920(3) 0.7567(3) 0.0314(13) Uani 1 1 d . . . . .
Na6 Na 0.6162(3) 0.2947(3) 0.4903(2) 0.0332(14) Uani 1 1 d . . . . .
Na7 Na 0.3875(4) 0.4147(5) 0.6902(4) 0.059(2) Uani 1 1 d . . . . .
O1 O 0.1182(5) 0.6377(5) 0.6231(4) 0.0195(19) Uani 1 1 d . . . . .
O1W O 0.4459(6) 0.7614(6) 0.8777(5) 0.034(2) Uani 1 1 d . . . . .
O2 O 0.3862(5) 0.3403(5) 0.8368(4) 0.022(2) Uani 1 1 d . . . . .
O2W O 0.5516(6) 0.7527(6) 0.9995(4) 0.032(2) Uani 1 1 d . . . . .
O3 O 0.2577(5) 0.8622(5) 0.7108(4) 0.0183(18) Uani 1 1 d . . . . .
O3W O 0.5103(6) 0.8952(6) 0.7754(5) 0.036(3) Uani 1 1 d . . . . .
O4 O 0.2386(5) 0.7251(5) 0.7372(4) 0.0197(19) Uani 1 1 d . . . . .
O4W O 0.4091(6) 0.9210(6) 0.9161(5) 0.034(2) Uani 1 1 d . . . . .
O5 O 0.1747(5) 0.6969(5) 0.5189(4) 0.0185(18) Uani 1 1 d . . . . .
O5W O 0.5810(6) 0.9087(6) 0.8995(5) 0.030(2) Uani 1 1 d . . . . .
O6 O 0.2424(5) 0.4496(5) 0.7991(4) 0.024(2) Uani 1 1 d . . . . .
O6W O 0.4762(6) 0.9293(6) 1.0433(5) 0.030(2) Uani 1 1 d . . . . .
O7 O 0.4145(5) 0.1897(5) 0.8863(4) 0.023(2) Uani 1 1 d . . . . .
O7W O 0.4626(6) 1.0509(6) 0.8215(6) 0.045(3) Uani 1 1 d . . . . .
O8 O 0.1168(5) 0.8537(5) 0.6895(4) 0.0168(18) Uani 1 1 d . . . . .
O8W O -0.0792(5) 1.0534(5) 0.4591(4) 0.027(2) Uani 1 1 d . . . . .
O9 O 0.2441(5) 0.5177(5) 0.6701(4) 0.0217(19) Uani 1 1 d . . . . .
O10 O 0.2412(5) 0.6671(5) 0.6349(4) 0.0176(18) Uani 1 1 d . . . . .
O11 O 0.2704(5) 0.2972(5) 0.8349(4) 0.0214(19) Uani 1 1 d . . . . .
O12 O 0.3772(5) 0.8345(5) 0.6249(4) 0.023(2) Uani 1 1 d . . . . .
O13 O 0.3779(5) 0.7339(5) 0.7478(4) 0.0210(19) Uani 1 1 d . . . . .
O14 O 0.1116(5) 0.7071(5) 0.7178(4) 0.0211(19) Uani 1 1 d . . . . .
O15 O 0.3980(5) 0.8674(5) 0.7345(4) 0.026(2) Uani 1 1 d . . . . .
O16 O 0.6358(5) 0.6772(5) 0.6807(4) 0.024(2) Uani 1 1 d . . . . .
O17 O 0.1884(5) 0.5511(5) 0.5471(4) 0.0208(19) Uani 1 1 d . . . . .
O18 O 0.1276(5) 0.4798(5) 0.6517(4) 0.024(2) Uani 1 1 d . . . . .
O19 O 0.1113(5) 0.5580(5) 0.7446(4) 0.023(2) Uani 1 1 d . . . . .
O20 O 0.2571(5) 0.3647(5) 0.7097(4) 0.023(2) Uani 1 1 d . . . . .
O21 O 0.3245(5) 0.6687(5) 0.8544(4) 0.025(2) Uani 1 1 d . . . . .
O22 O 0.5393(5) 0.1482(5) 0.8079(4) 0.024(2) Uani 1 1 d . . . . .
O23 O 0.5117(5) 0.2962(5) 0.7450(4) 0.022(2) Uani 1 1 d . . . . .
O24 O 0.1704(5) 0.9647(5) 0.6270(4) 0.024(2) Uani 1 1 d . . . . .
O25 O 0.1136(5) 0.7916(5) 0.5922(4) 0.0215(19) Uani 1 1 d . . . . .
O26 O 0.5208(5) 0.7278(5) 0.7642(4) 0.024(2) Uani 1 1 d . . . . .
O27 O 0.2955(5) 0.8364(5) 0.8255(4) 0.021(2) Uani 1 1 d . . . . .
O28 O 0.3418(5) 0.5337(5) 0.5783(4) 0.023(2) Uani 1 1 d . . . . .
O29 O 0.2967(5) 0.9738(5) 0.6547(5) 0.025(2) Uani 1 1 d . . . . .
O30 O 0.1277(5) 0.4061(5) 0.7844(4) 0.023(2) Uani 1 1 d . . . . .
O31 O 0.3204(5) 0.1571(5) 0.8325(4) 0.025(2) Uani 1 1 d . . . . .
O32 O 0.2435(5) 0.8176(5) 0.6081(4) 0.024(2) Uani 1 1 d . . . . .
O33 O 0.3955(5) 0.2460(5) 0.7581(5) 0.027(2) Uani 1 1 d . . . . .
O34 O 0.5200(6) 0.8271(5) 0.6492(4) 0.027(2) Uani 1 1 d . . . . .
O35 O 0.4978(5) 0.6964(5) 0.6521(4) 0.022(2) Uani 1 1 d . . . . .
O36 O 0.1617(5) 0.8404(5) 0.8017(4) 0.0210(19) Uani 1 1 d . . . . .
O37 O 0.0436(5) 1.0184(6) 0.6953(5) 0.029(2) Uani 1 1 d . . . . .
O38 O 0.1921(5) 0.2585(5) 0.7790(5) 0.027(2) Uani 1 1 d . . . . .
O39 O 0.2039(5) 0.2217(5) 0.9159(5) 0.026(2) Uani 1 1 d . . . . .
O40 O -0.0180(5) 0.8411(6) 0.5182(5) 0.027(2) Uani 1 1 d . . . . .
O41 O 0.5308(5) 0.2447(5) 0.8791(4) 0.023(2) Uani 1 1 d . . . . .
O42 O -0.0037(5) 0.7458(5) 0.6350(4) 0.024(2) Uani 1 1 d . . . . .
O43 O 0.0039(5) 0.6020(5) 0.6527(4) 0.024(2) Uani 1 1 d . . . . .
O44 O 0.0393(5) 0.6714(5) 0.5276(4) 0.025(2) Uani 1 1 d . . . . .
O45 O -0.0078(6) 0.6864(6) 0.7821(5) 0.030(2) Uani 1 1 d . . . . .
O46 O 0.6142(5) 0.5511(5) 0.6738(4) 0.023(2) Uani 1 1 d . . . . .
O47 O 0.3054(5) 0.2855(5) 0.9472(4) 0.024(2) Uani 1 1 d . . . . .
O48 O 0.0381(5) 0.9712(6) 0.7616(5) 0.031(2) Uani 1 1 d . . . . .
O49 O 0.3136(6) 1.0177(6) 0.7590(5) 0.037(3) Uani 1 1 d . . . . .
O50 O 0.7348(5) 0.6429(5) 0.7588(5) 0.026(2) Uani 1 1 d . . . . .
O51 O 0.3159(5) 0.6038(5) 0.5244(4) 0.026(2) Uani 1 1 d . . . . .
O52 O 0.1688(5) 0.3797(5) 0.9010(4) 0.023(2) Uani 1 1 d . . . . .
O53 O 0.0108(5) 0.5315(6) 0.5597(5) 0.029(2) Uani 1 1 d . . . . .
O54 O 0.6482(5) 0.1081(5) 0.8869(4) 0.026(2) Uani 1 1 d . . . . .
O55 O 0.6239(5) 0.5741(5) 0.7887(4) 0.023(2) Uani 1 1 d . . . . .
O56 O 0.6232(5) 0.1716(5) 0.7019(4) 0.027(2) Uani 1 1 d . . . . .
O57 O 0.1852(5) 0.9787(5) 0.7535(5) 0.028(2) Uani 1 1 d . . . . .
O58 O 0.0492(5) 0.8195(6) 0.4721(4) 0.027(2) Uani 1 1 d . . . . .
O59 O 0.6206(5) 0.3615(5) 0.7179(4) 0.027(2) Uani 1 1 d . . . . .
O60 O 0.2978(5) 0.9762(6) 0.5340(5) 0.029(2) Uani 1 1 d . . . . .
O61 O 0.7290(6) 0.2292(6) 0.6890(5) 0.031(2) Uani 1 1 d . . . . .
O62 O 0.6492(5) 0.2169(5) 0.7908(4) 0.025(2) Uani 1 1 d . . . . .
O63 O 0.7456(5) 0.5241(5) 0.7155(5) 0.027(2) Uani 1 1 d . . . . .
O64 O 0.8640(6) 0.5972(7) 0.6883(5) 0.038(3) Uani 1 1 d . . . . .
O65 O 0.7156(6) 0.6092(6) 0.5964(5) 0.031(2) Uani 1 1 d . . . . .
O66 O 0.3095(6) 0.9665(6) 0.8234(5) 0.031(2) Uani 1 1 d . . . . .
O67 O 0.6262(6) 0.7245(6) 0.8500(5) 0.029(2) Uani 1 1 d . . . . .
O68 O 0.3237(5) 0.4373(6) 0.9095(5) 0.028(2) Uani 1 1 d . . . . .
O69 O -0.0476(6) 0.6501(6) 0.7554(5) 0.034(2) Uani 1 1 d . . . . .
O70 O 0.7351(6) 0.7280(6) 0.6254(5) 0.031(2) Uani 1 1 d . . . . .
O71 O 0.2430(5) 0.7095(6) 0.8733(4) 0.027(2) Uani 1 1 d . . . . .
O72 O 0.7519(6) 0.2928(6) 0.7729(5) 0.033(2) Uani 1 1 d . . . . .
O73 O 0.6329(5) 0.7864(6) 0.7245(5) 0.029(2) Uani 1 1 d . . . . .
O74 O 0.6277(5) 0.3294(5) 0.8464(4) 0.027(2) Uani 1 1 d . . . . .
O75 O 0.6044(5) 0.7449(5) 0.5647(4) 0.026(2) Uani 1 1 d . . . . .
O76 O 0.8553(6) 0.5778(7) 0.6283(6) 0.041(3) Uani 1 1 d . . . . .
O77 O 0.7538(5) 0.0931(6) 0.7823(5) 0.031(2) Uani 1 1 d . . . . .
O78 O 0.5441(7) 0.3347(7) 0.6237(5) 0.044(3) Uani 1 1 d . . . . .
O79 O 0.6695(6) 0.4372(6) 0.7737(5) 0.031(2) Uani 1 1 d . . . . .
O80 O 0.3249(6) 0.1391(6) 1.0033(5) 0.030(2) Uani 1 1 d . . . . .
O81 O 0.6212(6) 0.6469(5) 0.8742(5) 0.031(2) Uani 1 1 d . . . . .
O82 O 0.6278(7) 0.3099(6) 0.6034(4) 0.037(3) Uani 1 1 d . . . . .
O83 O 0.3023(6) 0.2458(5) 0.6612(5) 0.031(2) Uani 1 1 d . . . . .
O84 O 0.6135(6) 0.6035(6) 0.5346(5) 0.035(2) Uani 1 1 d . . . . .
O85 O 0.6373(6) 0.1740(6) 0.9827(5) 0.034(2) Uani 1 1 d . . . . .
O86 O 0.7446(5) 0.1811(5) 0.8729(5) 0.028(2) Uani 1 1 d . . . . .
O87 O 0.0822(5) 0.5139(6) 0.5181(5) 0.031(2) Uani 1 1 d . . . . .
O88 O 0.3404(6) 0.0891(5) 0.9590(5) 0.033(2) Uani 1 1 d . . . . .
O89 O 0.2754(6) 0.9191(6) 0.5151(5) 0.031(2) Uani 1 1 d . . . . .
O90 O 0.0522(6) 0.3371(6) 0.8940(5) 0.033(2) Uani 1 1 d . . . . .
O91 O 0.3214(6) 0.1693(6) 0.7078(5) 0.036(3) Uani 1 1 d . . . . .
O92 O 0.0617(6) 0.2872(7) 0.8490(5) 0.039(3) Uani 1 1 d . . . . .
O93 O 0.6233(6) 0.2584(6) 0.9663(5) 0.032(2) Uani 1 1 d . . . . .
O94 O 0.6626(7) -0.0013(6) 0.8261(6) 0.042(3) Uani 1 1 d . . . . .
O95 O 0.2430(5) 0.4523(6) 0.9304(5) 0.029(2) Uani 1 1 d . . . . .
O96 O 0.6553(6) 0.0241(6) 0.7549(5) 0.039(3) Uani 1 1 d . . . . .
O97 O 0.6430(7) 0.8867(6) 0.6121(5) 0.043(3) Uani 1 1 d . . . . .
O98 O 0.5315(6) 0.6397(7) 0.5507(5) 0.038(3) Uani 1 1 d . . . . .
O99 O 0.8689(6) 0.1581(7) 0.7351(5) 0.039(3) Uani 1 1 d . . . . .
O100 O 0.8747(6) 0.1376(7) 0.8062(6) 0.042(3) Uani 1 1 d . . . . .
O101 O 0.6253(7) 0.8743(6) 0.5514(5) 0.044(3) Uani 1 1 d . . . . .
Na8 Na -0.0264(5) 0.4805(5) 0.7940(5) 0.076(3) Uani 1 1 d . . . . .
Na9 Na 0.7736(5) 0.8666(6) 0.5249(5) 0.095(4) Uani 1 1 d . . . . .
O10W O 0.0660(6) 0.5256(6) 0.8691(5) 0.036(3) Uani 1 1 d . . . . .
O11W O -0.0286(5) 0.8791(5) 0.6663(4) 0.022(2) Uani 1 1 d . . . . .
Na11 Na -0.0621(5) 0.4442(6) 0.6087(5) 0.083(3) Uani 1 1 d . U . . .
O13W O 0.4732(6) 0.5893(6) 0.8031(5) 0.033(2) Uani 1 1 d . . . . .
O14W O 0.3393(6) 0.5496(6) 0.8063(5) 0.038(3) Uani 1 1 d . . . . .
O15W O 0.7808(7) 0.1070(6) 0.6282(5) 0.040(3) Uani 1 1 d . . . . .
O16W O -0.0670(6) 1.0569(6) 0.6104(5) 0.034(2) Uani 1 1 d . . . . .
O17W O 0.4768(6) 0.4172(6) 0.8550(6) 0.041(3) Uani 1 1 d . . . . .
O18W O 0.7887(6) 0.4725(6) 0.5720(5) 0.039(3) Uani 1 1 d . . . . .
O19W O 0.4374(6) 0.0479(6) 0.6946(6) 0.042(3) Uani 1 1 d . . . . .
O20W O 0.7991(7) 0.3144(7) 0.6070(5) 0.047(3) Uani 1 1 d . . . . .
O21W O -0.1745(6) 0.9593(6) 0.5688(5) 0.036(2) Uani 1 1 d . . . . .
O22W O 0.7535(7) 0.2062(6) 0.5121(5) 0.041(3) Uani 1 1 d . . . . .
O23W O -0.1074(6) 0.9811(6) 0.7723(6) 0.039(3) Uani 1 1 d . . . . .
O24W O -0.0945(7) 0.8209(6) 0.8030(6) 0.047(3) Uani 1 1 d . . . . .
O25W O 0.6027(6) 0.3665(7) 0.3660(6) 0.047(3) Uani 1 1 d . . . . .
O26W O 0.1744(6) 0.6094(7) 0.8634(5) 0.042(3) Uani 1 1 d . . . . .
Na10 Na 0.2699(9) 0.3922(7) 0.5775(6) 0.123(4) Uani 1 1 d . U . . .
O28W O 0.4100(6) 0.3484(8) 0.5988(5) 0.051(3) Uani 1 1 d . . . . .
O29W O 0.0628(7) 0.7664(8) 0.8304(7) 0.055(3) Uani 1 1 d . . . . .
O30W O 0.2696(6) 0.2660(7) 1.0752(5) 0.040(3) Uani 1 1 d . . . . .
O31W O 0.1151(7) 0.3495(8) 1.0284(6) 0.057(4) Uani 1 1 d . . . . .
O32W O 0.1209(7) 1.1160(7) 0.5749(6) 0.054(3) Uani 1 1 d . . . . .
O33W O 0.4996(7) 0.5151(9) 0.5577(7) 0.062(4) Uani 1 1 d . . . . .
O34W O -0.2272(6) 0.8568(7) 0.8698(6) 0.053(3) Uani 1 1 d . . . . .
O35W O -0.1759(8) 0.6698(11) 0.8209(6) 0.074(5) Uani 1 1 d . . . . .
O36W O 0.7474(7) -0.0155(8) 0.9611(6) 0.058(4) Uani 1 1 d . . . . .
O37W O 0.2247(8) 1.0591(7) 0.9075(7) 0.064(4) Uani 1 1 d . U . . .
O38W O 0.7906(7) -0.0561(9) 0.7016(6) 0.060(4) Uani 1 1 d . . . . .
O39W O 0.7565(10) 0.8142(10) 0.7350(7) 0.079(5) Uani 1 1 d . . . . .
O40W O 0.4887(8) 0.1726(9) 0.6674(7) 0.070(5) Uani 1 1 d . . . . .
O41W O 0.2412(10) 0.4291(10) 1.0595(7) 0.080(5) Uani 1 1 d . . . . .
O42W O 0.4402(9) -0.0222(8) 0.6075(9) 0.082(5) Uani 1 1 d . U . . .
O43W O 0.1296(9) 0.2049(9) 1.0296(7) 0.074(5) Uani 1 1 d . . . . .
O44W O 0.8413(8) 0.3777(9) 0.7053(9) 0.082(5) Uani 1 1 d . . . . .
O45W O 0.500000 1.000000 0.500000 0.091(7) Uani 1 2 d S TU P . .
O46W O 0.8429(8) 0.7988(10) 0.6251(10) 0.089(6) Uani 1 1 d . . . . .
O47W O 0.2112(10) 0.1095(8) 0.8270(9) 0.083(5) Uani 1 1 d . U . . .
O48W O 0.0393(9) 0.5757(10) 0.9778(9) 0.086(5) Uani 1 1 d . . . . .
O49W O 0.4895(11) 0.4898(9) 0.7075(7) 0.086(5) Uani 1 1 d . U . . .
O50W O 0.2577(11) 0.2897(13) 0.5238(8) 0.097(6) Uani 1 1 d . U . . .
O51W O 0.2423(8) 0.8752(13) 0.9398(7) 0.097(7) Uani 1 1 d . . . . .
O52W O 0.8872(9) 0.6987(11) 0.5304(10) 0.095(6) Uani 1 1 d . . . . .
O53W O 0.4727(12) 0.5562(13) 0.9349(9) 0.109(6) Uani 1 1 d . U . . .
O54W O 0.6295(11) 0.1281(12) 0.5895(9) 0.098(6) Uani 1 1 d . U . . .
O55W O -0.1005(13) 0.9392(13) 0.9059(10) 0.116(7) Uiso 1 1 d . . . . .
O56W O 0.6207(13) 0.4512(14) 0.9061(11) 0.126(8) Uiso 1 1 d . . . . .
O57W O 0.5889(12) 0.8263(13) 0.4367(10) 0.112(7) Uiso 1 1 d . . . . .
O58W O 0.0411(14) 1.1049(15) 0.7835(12) 0.137(9) Uiso 1 1 d . . . . .
O12W O 0.2875(13) 0.6827(13) 0.9938(11) 0.120(7) Uiso 1 1 d . . . . .
O27W O 0.3699(14) 0.4984(14) 0.9876(12) 0.130(8) Uiso 1 1 d . . . . .
O9W O 0.0764(15) 0.4719(15) 1.0923(13) 0.144(9) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta2 3.2996(11) . ?
Ta1 Ta3 3.2654(10) . ?
Ta1 O61 2.109(10) . ?
Ta1 O62 2.186(10) . ?
Ta1 O72 2.017(10) . ?
Ta1 O77 1.936(10) . ?
Ta1 O86 1.988(10) . ?
Ta1 O99 1.965(10) . ?
Ta1 O100 1.958(11) . ?
Ta2 Ta4 3.2444(12) . ?
Ta2 O22 1.892(9) . ?
Ta2 O54 2.100(9) . ?
Ta2 O56 2.011(10) . ?
Ta2 O62 2.187(9) . ?
Ta2 O77 2.022(10) . ?
Ta2 O94 1.998(10) . ?
Ta2 O96 1.975(10) . ?
Ta3 O41 1.915(9) . ?
Ta3 O54 2.155(9) . ?
Ta3 O62 2.138(9) . ?
Ta3 O74 2.055(10) . ?
Ta3 O85 2.006(10) . ?
Ta3 O86 1.983(9) . ?
Ta3 O93 1.990(10) . ?
Ta4 K1 3.821(4) 2_666 ?
Ta4 O23 1.966(9) . ?
Ta4 O56 1.934(9) . ?
Ta4 O59 1.998(10) . ?
Ta4 O61 2.156(10) . ?
Ta4 O62 2.159(10) . ?
Ta4 O78 1.973(11) . ?
Ta4 O82 1.993(9) . ?
Ta5 Na7 3.606(8) . ?
Ta5 O2 1.931(9) . ?
Ta5 O7 1.982(9) . ?
Ta5 O22 2.021(9) . ?
Ta5 O23 1.945(9) . ?
Ta5 O33 1.992(10) . ?
Ta5 O41 2.013(9) . ?
Ta6 Ta8 3.2639(10) . ?
Ta6 O11 2.157(9) . ?
Ta6 O20 2.004(9) . ?
Ta6 O31 2.171(9) . ?
Ta6 O33 1.924(10) . ?
Ta6 O38 1.988(9) . ?
Ta6 O83 1.992(9) . ?
Ta6 O91 2.003(10) . ?
Ta7 Ta8 3.3060(11) . ?
Ta7 Ta9 3.2497(13) . ?
Ta7 O7 1.933(9) . ?
Ta7 O11 2.184(9) . ?
Ta7 O31 2.123(9) . ?
Ta7 O39 1.983(9) . ?
Ta7 O47 2.005(9) . ?
Ta7 O80 1.976(10) . ?
Ta7 O88 2.001(10) . ?
Ta8 O11 2.186(9) . ?
Ta8 O30 1.922(9) . ?
Ta8 O38 1.974(10) . ?
Ta8 O39 1.993(10) . ?
Ta8 O52 2.142(9) . ?
Ta8 O90 1.994(10) . ?
Ta8 O92 2.008(10) . ?
Ta9 O2 1.998(9) . ?
Ta9 O6 1.898(9) . ?
Ta9 O11 2.137(9) . ?
Ta9 O47 1.999(9) . ?
Ta9 O52 2.190(9) . ?
Ta9 O68 2.005(10) . ?
Ta9 O95 2.008(10) . ?
Ta10 Na5 3.274(6) . ?
Ta10 Na7 3.655(8) . ?
Ta10 O6 2.019(9) . ?
Ta10 O9 1.963(9) . ?
Ta10 O18 1.966(10) . ?
Ta10 O19 2.048(9) . ?
Ta10 O20 1.913(9) . ?
Ta10 O30 1.975(9) . ?
Ta10 Na10 3.719(11) . ?
Ta11 Ta13 3.2694(10) . ?
Ta11 Ta14 3.2998(13) . ?
Ta11 O1 2.210(9) . ?
Ta11 O17 1.984(9) . ?
Ta11 O18 1.940(9) . ?
Ta11 O43 2.090(9) . ?
Ta11 O44 2.005(9) . ?
Ta11 O53 1.993(9) . ?
Ta11 O87 1.975(9) . ?
Ta12 Ta14 3.2675(11) . ?
Ta12 Na5 3.523(6) . ?
Ta12 O1 2.120(9) . ?
Ta12 O14 2.102(9) . ?
Ta12 O19 1.900(9) . ?
Ta12 O42 1.990(9) . ?
Ta12 O43 2.104(9) . ?
Ta12 O45 1.990(9) . ?
Ta12 O69 1.969(10) . ?
Ta13 Na5 3.599(6) . ?
Ta13 O1 2.171(9) . ?
Ta13 O5 2.159(9) . ?
Ta13 O9 1.990(9) . ?
Ta13 O10 1.948(9) . ?
Ta13 O17 1.995(9) . ?
Ta13 O28 1.987(9) . ?
Ta13 O51 1.982(9) . ?
Ta14 O1 2.176(8) . ?
Ta14 O5 2.134(9) . ?
Ta14 O25 1.941(9) . ?
Ta14 O40 1.991(10) . ?
Ta14 O42 1.992(9) . ?
Ta14 O44 1.981(9) . ?
Ta14 O58 1.996(10) . ?
Ta15 Na5 3.360(6) . ?
Ta15 O4 1.976(9) . ?
Ta15 O8 1.953(8) . ?
Ta15 O10 1.992(9) . ?
Ta15 O14 2.201(9) . ?
Ta15 O25 1.953(9) . ?
Ta15 O32 1.902(10) . ?
Ta16 Ta19 3.2507(12) . ?
Ta16 O3 2.157(9) . ?
Ta16 O4 1.931(9) . ?
Ta16 O13 1.983(9) . ?
Ta16 O21 1.991(9) . ?
Ta16 O27 1.975(9) . ?
Ta16 O36 2.170(9) . ?
Ta16 O71 2.007(9) . ?
Ta17 Ta18 3.2674(10) . ?
Ta17 Ta19 3.2975(11) . ?
Ta17 O3 2.196(9) . ?
Ta17 O8 1.970(8) . ?
Ta17 O24 1.998(9) . ?
Ta17 O36 2.135(9) . ?
Ta17 O37 1.975(9) . ?
Ta17 O48 1.993(9) . ?
Ta17 O57 1.953(10) . ?
Ta18 O3 2.156(9) . ?
Ta18 O12 1.921(9) . ?
Ta18 O24 1.967(9) . ?
Ta18 O29 2.124(9) . ?
Ta18 O32 2.026(10) . ?
Ta18 O60 2.004(9) . ?
Ta18 O89 2.006(10) . ?
Ta19 O3 2.191(8) . ?
Ta19 O15 1.916(10) . ?
Ta19 O27 2.010(9) . ?
Ta19 O29 2.134(10) . ?
Ta19 O49 1.998(10) . ?
Ta19 O57 1.999(10) . ?
Ta19 O66 1.973(10) . ?
Ta20 O12 1.980(9) . ?
Ta20 O13 1.937(9) . ?
Ta20 O15 2.014(10) . ?
Ta20 O26 2.014(10) . ?
Ta20 O34 2.040(10) . ?
Ta20 O35 1.946(9) . ?
Ta21 Ta22 3.2366(12) . ?
Ta21 Ta24 3.2946(12) . ?
Ta21 O16 2.184(9) . ?
Ta21 O34 1.881(10) . ?
Ta21 O70 2.042(10) . ?
Ta21 O73 2.127(10) . ?
Ta21 O75 2.012(9) . ?
Ta21 O97 1.992(11) . ?
Ta21 O101 1.989(11) . ?
Ta22 K1 3.921(4) 2_666 ?
Ta22 O16 2.159(9) . ?
Ta22 O35 1.975(9) . ?
Ta22 O46 2.000(9) . ?
Ta22 O65 2.165(10) . ?
Ta22 O75 1.941(9) . ?
Ta22 O84 1.993(10) . ?
Ta22 O98 1.993(11) . ?
Ta23 Ta24 3.2726(10) . ?
Ta23 O16 2.150(9) . ?
Ta23 O26 1.911(9) . ?
Ta23 O50 1.986(9) . ?
Ta23 O55 2.061(9) . ?
Ta23 O67 1.994(9) . ?
Ta23 O73 2.170(10) . ?
Ta23 O81 1.996(10) . ?
Ta24 O16 2.186(9) . ?
Ta24 O50 1.980(9) . ?
Ta24 O63 2.060(10) . ?
Ta24 O64 1.980(10) . ?
Ta24 O65 2.108(10) . ?
Ta24 O70 1.909(10) . ?
Ta24 O76 1.985(10) . ?
K1 Na6 4.382(7) 2_666 ?
K1 O46 3.037(9) 2_666 ?
K1 O51 2.769(10) . ?
K1 O59 2.960(10) 2_666 ?
K1 O78 3.406(13) 2_666 ?
K1 O82 2.776(11) 2_666 ?
K1 O84 2.877(12) 2_666 ?
K1 O18W 2.945(12) 2_666 ?
K1 O20W 3.025(14) 2_666 ?
K1 O33W 2.775(15) 2_666 ?
Si1 O59 1.652(10) . ?
Si1 O72 1.622(11) . ?
Si1 O74 1.632(10) . ?
Si1 O79 1.630(10) . ?
Si2 O46 1.648(10) . ?
Si2 O55 1.635(10) . ?
Si2 O63 1.617(10) . ?
Si2 O79 1.609(10) . ?
Na1 Na2 3.661(9) . ?
Na1 O1W 2.725(13) . ?
Na1 O2W 2.648(12) . ?
Na1 O81 2.940(12) . ?
Na1 O93 2.808(12) 2_667 ?
Na1 O53W 2.68(2) . ?
Na1 O27W 2.91(3) 2_667 ?
Na2 Na3 3.444(8) . ?
Na2 O1W 2.453(12) . ?
Na2 O2W 2.484(11) . ?
Na2 O3W 2.458(12) . ?
Na2 O4W 2.398(12) . ?
Na2 O5W 2.357(11) . ?
Na2 O67 2.463(12) . ?
Na3 Na3 3.395(11) 2_677 ?
Na3 O4W 2.285(12) . ?
Na3 O5W 2.413(12) . ?
Na3 O6W 2.401(11) 2_677 ?
Na3 O6W 2.332(11) . ?
Na3 O7W 2.451(13) . ?
Na3 O88 2.487(12) 1_565 ?
Na4 Na4 3.442(11) 2_576 ?
Na4 O8W 2.392(11) . ?
Na4 O8W 2.448(11) 2_576 ?
Na4 O40 2.581(11) . ?
Na4 O11W 2.453(10) . ?
Na4 O16W 2.374(12) . ?
Na4 O21W 2.368(12) . ?
Na5 O4 2.670(10) . ?
Na5 O6 2.613(11) . ?
Na5 O9 2.609(10) . ?
Na5 O10 2.708(10) . ?
Na5 O14 2.508(11) . ?
Na5 O19 2.625(11) . ?
Na5 O14W 2.368(12) . ?
Na5 O26W 2.454(12) . ?
Na6 O51 2.744(12) 2_666 ?
Na6 O82 2.628(11) . ?
Na6 O98 2.820(12) 2_666 ?
Na6 O22W 2.581(14) . ?
Na6 O25W 2.695(14) . ?
Na7 O9 2.742(11) . ?
Na7 O20 3.010(12) . ?
Na7 O23 2.760(11) . ?
Na7 O28 2.851(12) . ?
Na7 Na10 3.833(18) . ?
Na7 O28W 2.584(16) . ?
O17 Na10 2.843(14) . ?
O20 Na10 2.782(15) . ?
O21 O71 1.521(13) . ?
O28 O51 1.512(13) . ?
O30 Na8 2.776(12) . ?
O37 O48 1.505(14) . ?
O40 O58 1.520(13) . ?
O45 O69 1.511(13) . ?
O49 O66 1.501(14) . ?
O53 O87 1.514(13) . ?
O53 Na11 2.573(13) . ?
O60 O89 1.535(13) . ?
O60 Na9 2.859(14) 2_676 ?
O64 O76 1.519(15) . ?
O67 O81 1.520(13) . ?
O68 O95 1.504(13) . ?
O76 Na11 2.615(15) 1_655 ?
O78 O82 1.537(16) . ?
O80 O88 1.493(14) . ?
O83 O91 1.511(14) . ?
O83 Na10 2.849(16) . ?
O84 O98 1.502(15) . ?
O85 O93 1.531(14) . ?
O87 Na11 2.708(15) 2_566 ?
O90 O92 1.528(15) . ?
O94 O96 1.508(16) . ?
O97 O101 1.530(16) . ?
O97 Na9 2.903(15) . ?
O99 O100 1.506(16) . ?
O101 Na9 2.812(15) . ?
Na8 O9W 2.81(3) 2_567 ?
Na9 O21W 2.846(17) 1_655 ?
Na9 O32W 2.809(17) 2_676 ?
Na9 O46W 2.50(2) . ?
Na11 O18W 2.930(15) 1_455 ?
Na11 O44W 2.994(19) 1_455 ?
Na10 O28W 2.59(2) . ?
Na10 O50W 2.72(2) . ?
O37W O47W 1.77(2) 1_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ta3 Ta1 Ta2 62.86(2) . . ?
O61 Ta1 Ta2 78.3(3) . . ?
O61 Ta1 Ta3 110.5(3) . . ?
O61 Ta1 O62 72.1(4) . . ?
O62 Ta1 Ta2 41.0(2) . . ?
O62 Ta1 Ta3 40.4(2) . . ?
O72 Ta1 Ta2 127.0(3) . . ?
O72 Ta1 Ta3 80.3(3) . . ?
O72 Ta1 O61 80.9(4) . . ?
O72 Ta1 O62 86.2(4) . . ?
O77 Ta1 Ta2 34.4(3) . . ?
O77 Ta1 Ta3 89.1(3) . . ?
O77 Ta1 O61 87.8(4) . . ?
O77 Ta1 O62 75.4(4) . . ?
O77 Ta1 O72 160.7(4) . . ?
O77 Ta1 O86 96.6(4) . . ?
O77 Ta1 O99 97.6(4) . . ?
O77 Ta1 O100 100.0(5) . . ?
O86 Ta1 Ta2 85.6(3) . . ?
O86 Ta1 Ta3 34.6(3) . . ?
O86 Ta1 O61 144.2(4) . . ?
O86 Ta1 O62 74.8(4) . . ?
O86 Ta1 O72 83.9(4) . . ?
O99 Ta1 Ta2 128.3(3) . . ?
O99 Ta1 Ta3 164.4(3) . . ?
O99 Ta1 O61 83.9(4) . . ?
O99 Ta1 O62 155.1(4) . . ?
O99 Ta1 O72 96.7(5) . . ?
O99 Ta1 O86 130.1(4) . . ?
O100 Ta1 Ta2 131.3(4) . . ?
O100 Ta1 Ta3 119.9(3) . . ?
O100 Ta1 O61 129.0(4) . . ?
O100 Ta1 O62 158.7(4) . . ?
O100 Ta1 O72 99.3(5) . . ?
O100 Ta1 O86 85.3(4) . . ?
O100 Ta1 O99 45.2(5) . . ?
Ta4 Ta2 Ta1 64.16(2) . . ?
O22 Ta2 Ta1 130.9(3) . . ?
O22 Ta2 Ta4 81.9(3) . . ?
O22 Ta2 O54 83.9(4) . . ?
O22 Ta2 O56 86.2(4) . . ?
O22 Ta2 O62 90.1(4) . . ?
O22 Ta2 O77 163.1(4) . . ?
O22 Ta2 O94 98.6(4) . . ?
O22 Ta2 O96 100.9(4) . . ?
O54 Ta2 Ta1 78.4(3) . . ?
O54 Ta2 Ta4 112.7(3) . . ?
O54 Ta2 O62 73.4(4) . . ?
O56 Ta2 Ta1 84.2(3) . . ?
O56 Ta2 Ta4 33.9(3) . . ?
O56 Ta2 O54 146.4(4) . . ?
O56 Ta2 O62 74.6(4) . . ?
O56 Ta2 O77 93.9(4) . . ?
O62 Ta2 Ta1 41.0(2) . . ?
O62 Ta2 Ta4 41.4(3) . . ?
O77 Ta2 Ta1 32.7(3) . . ?
O77 Ta2 Ta4 88.7(3) . . ?
O77 Ta2 O54 86.8(4) . . ?
O77 Ta2 O62 73.7(4) . . ?
O94 Ta2 Ta1 124.3(3) . . ?
O94 Ta2 Ta4 162.8(3) . . ?
O94 Ta2 O54 84.4(4) . . ?
O94 Ta2 O56 128.9(4) . . ?
O94 Ta2 O62 155.2(4) . . ?
O94 Ta2 O77 94.5(4) . . ?
O96 Ta2 Ta1 125.8(3) . . ?
O96 Ta2 Ta4 118.3(3) . . ?
O96 Ta2 O54 129.0(4) . . ?
O96 Ta2 O56 84.4(4) . . ?
O96 Ta2 O62 155.6(4) . . ?
O96 Ta2 O77 96.0(4) . . ?
O96 Ta2 O94 44.6(5) . . ?
O41 Ta3 Ta1 126.9(3) . . ?
O41 Ta3 O54 84.7(4) . . ?
O41 Ta3 O62 85.5(4) . . ?
O41 Ta3 O74 93.3(4) . . ?
O41 Ta3 O85 98.1(4) . . ?
O41 Ta3 O86 159.9(4) . . ?
O41 Ta3 O93 98.1(4) . . ?
O54 Ta3 Ta1 78.5(2) . . ?
O62 Ta3 Ta1 41.5(3) . . ?
O62 Ta3 O54 73.3(3) . . ?
O74 Ta3 Ta1 81.6(3) . . ?
O74 Ta3 O54 153.3(4) . . ?
O74 Ta3 O62 79.9(4) . . ?
O85 Ta3 Ta1 127.7(3) . . ?
O85 Ta3 O54 81.1(4) . . ?
O85 Ta3 O62 153.8(4) . . ?
O85 Ta3 O74 125.4(4) . . ?
O86 Ta3 Ta1 34.7(3) . . ?
O86 Ta3 O54 82.6(4) . . ?
O86 Ta3 O62 76.0(4) . . ?
O86 Ta3 O74 91.1(4) . . ?
O86 Ta3 O85 95.3(4) . . ?
O86 Ta3 O93 102.0(4) . . ?
O93 Ta3 Ta1 132.2(3) . . ?
O93 Ta3 O54 126.1(4) . . ?
O93 Ta3 O62 160.4(4) . . ?
O93 Ta3 O74 80.6(4) . . ?
O93 Ta3 O85 45.0(4) . . ?
Ta2 Ta4 K1 157.57(6) . 2_666 ?
O23 Ta4 Ta2 82.0(3) . . ?
O23 Ta4 K1 117.7(3) . 2_666 ?
O23 Ta4 O59 90.4(4) . . ?
O23 Ta4 O61 153.1(4) . . ?
O23 Ta4 O62 81.4(4) . . ?
O23 Ta4 O78 82.7(4) . . ?
O23 Ta4 O82 128.3(4) . . ?
O56 Ta4 Ta2 35.5(3) . . ?
O56 Ta4 K1 141.9(3) . 2_666 ?
O56 Ta4 O23 94.0(4) . . ?
O56 Ta4 O59 157.9(4) . . ?
O56 Ta4 O61 81.5(4) . . ?
O56 Ta4 O62 76.8(4) . . ?
O56 Ta4 O78 104.3(5) . . ?
O56 Ta4 O82 99.8(4) . . ?
O59 Ta4 Ta2 124.5(3) . . ?
O59 Ta4 K1 49.9(3) . 2_666 ?
O59 Ta4 O61 84.9(4) . . ?
O59 Ta4 O62 82.5(4) . . ?
O61 Ta4 Ta2 79.1(3) . . ?
O61 Ta4 K1 78.7(3) . 2_666 ?
O61 Ta4 O62 71.7(4) . . ?
O62 Ta4 Ta2 42.0(2) . . ?
O62 Ta4 K1 125.8(3) . 2_666 ?
O78 Ta4 Ta2 134.9(4) . . ?
O78 Ta4 K1 62.8(4) . 2_666 ?
O78 Ta4 O59 97.7(5) . . ?
O78 Ta4 O61 124.2(4) . . ?
O78 Ta4 O62 164.1(4) . . ?
O78 Ta4 O82 45.6(5) . . ?
O82 Ta4 Ta2 132.4(3) . . ?
O82 Ta4 K1 44.5(3) . 2_666 ?
O82 Ta4 O59 94.4(4) . . ?
O82 Ta4 O61 78.5(4) . . ?
O82 Ta4 O62 150.3(4) . . ?
O2 Ta5 Na7 60.4(3) . . ?
O2 Ta5 O7 88.6(4) . . ?
O2 Ta5 O22 173.7(4) . . ?
O2 Ta5 O23 98.0(4) . . ?
O2 Ta5 O33 91.8(4) . . ?
O2 Ta5 O41 91.3(4) . . ?
O7 Ta5 Na7 133.4(3) . . ?
O7 Ta5 O22 86.1(4) . . ?
O7 Ta5 O33 87.1(4) . . ?
O7 Ta5 O41 91.0(4) . . ?
O22 Ta5 Na7 126.0(3) . . ?
O23 Ta5 Na7 49.2(3) . . ?
O23 Ta5 O7 172.5(4) . . ?
O23 Ta5 O22 87.5(4) . . ?
O23 Ta5 O33 89.1(4) . . ?
O23 Ta5 O41 92.3(4) . . ?
O33 Ta5 Na7 62.4(3) . . ?
O33 Ta5 O22 91.4(4) . . ?
O33 Ta5 O41 176.3(4) . . ?
O41 Ta5 Na7 121.0(3) . . ?
O41 Ta5 O22 85.3(4) . . ?
O11 Ta6 Ta8 41.6(2) . . ?
O11 Ta6 O31 72.8(3) . . ?
O20 Ta6 Ta8 80.4(3) . . ?
O20 Ta6 O11 80.7(3) . . ?
O20 Ta6 O31 153.4(4) . . ?
O31 Ta6 Ta8 78.5(3) . . ?
O33 Ta6 Ta8 126.0(3) . . ?
O33 Ta6 O11 84.4(4) . . ?
O33 Ta6 O20 94.9(4) . . ?
O33 Ta6 O31 84.6(4) . . ?
O33 Ta6 O38 157.8(4) . . ?
O33 Ta6 O83 99.9(4) . . ?
O33 Ta6 O91 98.0(4) . . ?
O38 Ta6 Ta8 34.4(3) . . ?
O38 Ta6 O11 75.4(4) . . ?
O38 Ta6 O20 91.0(4) . . ?
O38 Ta6 O31 80.6(4) . . ?
O38 Ta6 O83 102.1(4) . . ?
O38 Ta6 O91 95.5(4) . . ?
O83 Ta6 Ta8 131.9(3) . . ?
O83 Ta6 O11 162.9(4) . . ?
O83 Ta6 O20 82.5(4) . . ?
O83 Ta6 O31 123.9(4) . . ?
O83 Ta6 O91 44.4(4) . . ?
O91 Ta6 Ta8 127.8(3) . . ?
O91 Ta6 O11 151.8(4) . . ?
O91 Ta6 O20 126.7(4) . . ?
O91 Ta6 O31 79.5(4) . . ?
Ta9 Ta7 Ta8 63.97(2) . . ?
O7 Ta7 Ta8 131.0(3) . . ?
O7 Ta7 Ta9 82.7(3) . . ?
O7 Ta7 O11 90.4(4) . . ?
O7 Ta7 O31 82.7(4) . . ?
O7 Ta7 O39 163.5(4) . . ?
O7 Ta7 O47 86.4(4) . . ?
O7 Ta7 O80 101.8(4) . . ?
O7 Ta7 O88 95.0(4) . . ?
O11 Ta7 Ta8 40.9(2) . . ?
O11 Ta7 Ta9 40.7(2) . . ?
O31 Ta7 Ta8 78.1(3) . . ?
O31 Ta7 Ta9 111.6(2) . . ?
O31 Ta7 O11 73.2(3) . . ?
O39 Ta7 Ta8 33.8(3) . . ?
O39 Ta7 Ta9 90.3(3) . . ?
O39 Ta7 O11 74.7(3) . . ?
O39 Ta7 O31 86.1(4) . . ?
O39 Ta7 O47 96.7(4) . . ?
O39 Ta7 O88 95.6(4) . . ?
O47 Ta7 Ta8 85.9(3) . . ?
O47 Ta7 Ta9 35.7(3) . . ?
O47 Ta7 O11 75.8(4) . . ?
O47 Ta7 O31 146.9(3) . . ?
O80 Ta7 Ta8 125.7(3) . . ?
O80 Ta7 Ta9 121.5(3) . . ?
O80 Ta7 O11 157.3(4) . . ?
O80 Ta7 O31 126.9(4) . . ?
O80 Ta7 O39 94.6(4) . . ?
O80 Ta7 O47 85.9(4) . . ?
O80 Ta7 O88 44.1(4) . . ?
O88 Ta7 Ta8 126.2(3) . . ?
O88 Ta7 Ta9 164.7(3) . . ?
O88 Ta7 O11 154.6(4) . . ?
O88 Ta7 O31 82.9(4) . . ?
O88 Ta7 O47 129.3(4) . . ?
Ta6 Ta8 Ta7 63.48(3) . . ?
O11 Ta8 Ta6 41.0(2) . . ?
O11 Ta8 Ta7 40.8(2) . . ?
O30 Ta8 Ta6 84.0(3) . . ?
O30 Ta8 Ta7 130.3(3) . . ?
O30 Ta8 O11 89.9(4) . . ?
O30 Ta8 O38 88.6(4) . . ?
O30 Ta8 O39 162.9(4) . . ?
O30 Ta8 O52 80.9(4) . . ?
O30 Ta8 O90 96.1(4) . . ?
O30 Ta8 O92 101.1(4) . . ?
O38 Ta8 Ta6 34.7(3) . . ?
O38 Ta8 Ta7 84.7(3) . . ?
O38 Ta8 O11 75.1(4) . . ?
O38 Ta8 O39 94.1(4) . . ?
O38 Ta8 O52 145.9(4) . . ?
O38 Ta8 O90 130.0(4) . . ?
O38 Ta8 O92 85.3(4) . . ?
O39 Ta8 Ta6 88.6(3) . . ?
O39 Ta8 Ta7 33.7(3) . . ?
O39 Ta8 O11 74.5(3) . . ?
O39 Ta8 O52 87.5(4) . . ?
O39 Ta8 O90 95.1(4) . . ?
O39 Ta8 O92 96.0(4) . . ?
O52 Ta8 Ta6 111.6(2) . . ?
O52 Ta8 Ta7 78.0(2) . . ?
O52 Ta8 O11 72.6(3) . . ?
O90 Ta8 Ta6 164.6(3) . . ?
O90 Ta8 Ta7 125.1(3) . . ?
O90 Ta8 O11 154.2(4) . . ?
O90 Ta8 O52 83.6(4) . . ?
O90 Ta8 O92 44.9(4) . . ?
O92 Ta8 Ta6 119.9(3) . . ?
O92 Ta8 Ta7 127.2(3) . . ?
O92 Ta8 O11 157.2(4) . . ?
O92 Ta8 O52 128.5(4) . . ?
O2 Ta9 Ta7 81.4(2) . . ?
O2 Ta9 O11 82.3(3) . . ?
O2 Ta9 O47 91.8(4) . . ?
O2 Ta9 O52 154.9(4) . . ?
O2 Ta9 O68 82.6(4) . . ?
O2 Ta9 O95 126.6(4) . . ?
O6 Ta9 Ta7 127.4(3) . . ?
O6 Ta9 O2 94.0(4) . . ?
O6 Ta9 O11 85.6(4) . . ?
O6 Ta9 O47 160.8(4) . . ?
O6 Ta9 O52 86.1(4) . . ?
O6 Ta9 O68 100.1(4) . . ?
O6 Ta9 O95 95.5(4) . . ?
O11 Ta9 Ta7 41.8(2) . . ?
O11 Ta9 O52 72.6(3) . . ?
O47 Ta9 Ta7 35.8(3) . . ?
O47 Ta9 O11 77.0(3) . . ?
O47 Ta9 O52 81.0(3) . . ?
O47 Ta9 O68 98.9(4) . . ?
O47 Ta9 O95 95.7(4) . . ?
O52 Ta9 Ta7 78.7(2) . . ?
O68 Ta9 Ta7 130.6(3) . . ?
O68 Ta9 O11 164.2(4) . . ?
O68 Ta9 O52 122.2(4) . . ?
O68 Ta9 O95 44.0(4) . . ?
O95 Ta9 Ta7 128.9(3) . . ?
O95 Ta9 O11 150.7(4) . . ?
O95 Ta9 O52 78.2(4) . . ?
Na5 Ta10 Na7 73.16(17) . . ?
Na5 Ta10 Na10 120.1(3) . . ?
Na7 Ta10 Na10 62.6(3) . . ?
O6 Ta10 Na5 52.9(3) . . ?
O6 Ta10 Na7 66.2(3) . . ?
O6 Ta10 O19 86.1(4) . . ?
O6 Ta10 Na10 126.9(4) . . ?
O9 Ta10 Na5 52.8(3) . . ?
O9 Ta10 Na7 47.5(3) . . ?
O9 Ta10 O6 88.2(4) . . ?
O9 Ta10 O18 89.8(4) . . ?
O9 Ta10 O19 88.3(4) . . ?
O9 Ta10 O30 175.0(4) . . ?
O9 Ta10 Na10 67.5(4) . . ?
O18 Ta10 Na5 121.8(3) . . ?
O18 Ta10 Na7 116.1(3) . . ?
O18 Ta10 O6 174.1(4) . . ?
O18 Ta10 O19 88.3(4) . . ?
O18 Ta10 O30 93.2(4) . . ?
O18 Ta10 Na10 57.0(4) . . ?
O19 Ta10 Na5 53.3(3) . . ?
O19 Ta10 Na7 125.6(3) . . ?
O19 Ta10 Na10 135.9(3) . . ?
O20 Ta10 Na5 127.1(3) . . ?
O20 Ta10 Na7 55.3(3) . . ?
O20 Ta10 O6 92.2(4) . . ?
O20 Ta10 O9 93.8(4) . . ?
O20 Ta10 O18 93.4(4) . . ?
O20 Ta10 O19 177.3(4) . . ?
O20 Ta10 O30 90.0(4) . . ?
O20 Ta10 Na10 46.7(3) . . ?
O30 Ta10 Na5 122.1(3) . . ?
O30 Ta10 Na7 133.7(3) . . ?
O30 Ta10 O6 88.4(4) . . ?
O30 Ta10 O19 87.8(4) . . ?
O30 Ta10 Na10 117.6(4) . . ?
Ta13 Ta11 Ta14 63.718(19) . . ?
O1 Ta11 Ta13 41.3(2) . . ?
O1 Ta11 Ta14 40.8(2) . . ?
O17 Ta11 Ta13 34.8(2) . . ?
O17 Ta11 Ta14 84.8(2) . . ?
O17 Ta11 O1 75.5(3) . . ?
O17 Ta11 O43 146.0(4) . . ?
O17 Ta11 O44 94.8(4) . . ?
O17 Ta11 O53 129.5(4) . . ?
O18 Ta11 Ta13 83.3(3) . . ?
O18 Ta11 Ta14 131.0(3) . . ?
O18 Ta11 O1 90.5(3) . . ?
O18 Ta11 O17 87.4(4) . . ?
O18 Ta11 O43 82.4(4) . . ?
O18 Ta11 O44 163.9(4) . . ?
O18 Ta11 O53 97.0(4) . . ?
O18 Ta11 O87 100.1(4) . . ?
O43 Ta11 Ta13 111.5(3) . . ?
O43 Ta11 Ta14 77.9(3) . . ?
O43 Ta11 O1 72.3(3) . . ?
O44 Ta11 Ta13 89.4(3) . . ?
O44 Ta11 Ta14 33.9(3) . . ?
O44 Ta11 O1 74.7(3) . . ?
O44 Ta11 O43 87.0(4) . . ?
O53 Ta11 Ta13 164.3(3) . . ?
O53 Ta11 Ta14 124.5(3) . . ?
O53 Ta11 O1 154.0(4) . . ?
O53 Ta11 O43 84.0(4) . . ?
O53 Ta11 O44 93.9(4) . . ?
O87 Ta11 Ta13 119.5(3) . . ?
O87 Ta11 Ta14 127.0(3) . . ?
O87 Ta11 O1 157.1(4) . . ?
O87 Ta11 O17 84.7(4) . . ?
O87 Ta11 O43 128.9(4) . . ?
O87 Ta11 O44 96.0(4) . . ?
O87 Ta11 O53 44.9(4) . . ?
Ta14 Ta12 Na5 101.02(10) . . ?
O1 Ta12 Ta14 41.1(2) . . ?
O1 Ta12 Na5 73.2(2) . . ?
O14 Ta12 Ta14 80.7(2) . . ?
O14 Ta12 Na5 44.6(3) . . ?
O14 Ta12 O1 81.5(3) . . ?
O14 Ta12 O43 155.2(3) . . ?
O19 Ta12 Ta14 125.4(3) . . ?
O19 Ta12 Na5 47.0(3) . . ?
O19 Ta12 O1 84.3(3) . . ?
O19 Ta12 O14 90.9(4) . . ?
O19 Ta12 O42 160.1(4) . . ?
O19 Ta12 O43 90.1(4) . . ?
O19 Ta12 O45 96.6(4) . . ?
O19 Ta12 O69 97.8(4) . . ?
O42 Ta12 Ta14 34.9(2) . . ?
O42 Ta12 Na5 125.6(3) . . ?
O42 Ta12 O1 75.8(3) . . ?
O42 Ta12 O14 87.6(4) . . ?
O42 Ta12 O43 83.2(4) . . ?
O43 Ta12 Ta14 78.6(3) . . ?
O43 Ta12 Na5 127.4(3) . . ?
O43 Ta12 O1 73.9(3) . . ?
O45 Ta12 Ta14 133.8(3) . . ?
O45 Ta12 Na5 94.4(3) . . ?
O45 Ta12 O1 162.1(4) . . ?
O45 Ta12 O14 80.6(4) . . ?
O45 Ta12 O42 102.6(4) . . ?
O45 Ta12 O43 123.9(4) . . ?
O69 Ta12 Ta14 130.7(3) . . ?
O69 Ta12 Na5 127.3(3) . . ?
O69 Ta12 O1 152.9(4) . . ?
O69 Ta12 O14 125.3(4) . . ?
O69 Ta12 O42 99.2(4) . . ?
O69 Ta12 O43 79.1(4) . . ?
O69 Ta12 O45 44.9(4) . . ?
Ta11 Ta13 Na5 100.13(9) . . ?
O1 Ta13 Ta11 42.2(2) . . ?
O1 Ta13 Na5 71.0(2) . . ?
O5 Ta13 Ta11 78.7(2) . . ?
O5 Ta13 Na5 123.9(2) . . ?
O5 Ta13 O1 72.5(3) . . ?
O9 Ta13 Ta11 81.6(3) . . ?
O9 Ta13 Na5 45.2(3) . . ?
O9 Ta13 O1 82.3(3) . . ?
O9 Ta13 O5 154.7(3) . . ?
O9 Ta13 O17 91.9(4) . . ?
O10 Ta13 Ta11 125.7(2) . . ?
O10 Ta13 Na5 47.8(3) . . ?
O10 Ta13 O1 83.5(3) . . ?
O10 Ta13 O5 87.1(3) . . ?
O10 Ta13 O9 91.7(4) . . ?
O10 Ta13 O17 158.7(3) . . ?
O10 Ta13 O28 102.1(4) . . ?
O10 Ta13 O51 97.4(4) . . ?
O17 Ta13 Ta11 34.6(3) . . ?
O17 Ta13 Na5 127.9(3) . . ?
O17 Ta13 O1 76.2(3) . . ?
O17 Ta13 O5 80.8(3) . . ?
O28 Ta13 Ta11 129.5(3) . . ?
O28 Ta13 Na5 100.5(3) . . ?
O28 Ta13 O1 162.9(3) . . ?
O28 Ta13 O5 123.5(3) . . ?
O28 Ta13 O9 81.4(4) . . ?
O28 Ta13 O17 99.2(4) . . ?
O51 Ta13 Ta11 129.6(3) . . ?
O51 Ta13 Na5 129.7(3) . . ?
O51 Ta13 O1 151.4(3) . . ?
O51 Ta13 O5 78.9(4) . . ?
O51 Ta13 O9 126.2(4) . . ?
O51 Ta13 O17 97.4(4) . . ?
O51 Ta13 O28 44.8(4) . . ?
Ta12 Ta14 Ta11 62.47(2) . . ?
O1 Ta14 Ta11 41.6(2) . . ?
O1 Ta14 Ta12 39.9(2) . . ?
O5 Ta14 Ta11 78.3(2) . . ?
O5 Ta14 Ta12 111.2(2) . . ?
O5 Ta14 O1 72.9(3) . . ?
O25 Ta14 Ta11 130.6(3) . . ?
O25 Ta14 Ta12 85.7(3) . . ?
O25 Ta14 O1 89.6(4) . . ?
O25 Ta14 O5 79.8(3) . . ?
O25 Ta14 O40 96.1(4) . . ?
O25 Ta14 O42 87.9(4) . . ?
O25 Ta14 O44 163.1(4) . . ?
O25 Ta14 O58 95.1(4) . . ?
O40 Ta14 Ta11 131.9(3) . . ?
O40 Ta14 Ta12 120.2(3) . . ?
O40 Ta14 O1 158.9(4) . . ?
O40 Ta14 O5 128.0(4) . . ?
O40 Ta14 O42 85.4(4) . . ?
O40 Ta14 O58 44.8(4) . . ?
O42 Ta14 Ta11 85.6(3) . . ?
O42 Ta14 Ta12 34.8(3) . . ?
O42 Ta14 O1 74.5(4) . . ?
O42 Ta14 O5 145.2(3) . . ?
O42 Ta14 O58 130.2(4) . . ?
O44 Ta14 Ta11 34.3(3) . . ?
O44 Ta14 Ta12 88.5(3) . . ?
O44 Ta14 O1 75.9(4) . . ?
O44 Ta14 O5 87.6(4) . . ?
O44 Ta14 O40 100.5(4) . . ?
O44 Ta14 O42 96.4(4) . . ?
O44 Ta14 O58 94.5(4) . . ?
O58 Ta14 Ta11 125.4(3) . . ?
O58 Ta14 Ta12 165.0(3) . . ?
O58 Ta14 O1 154.9(4) . . ?
O58 Ta14 O5 83.6(4) . . ?
O4 Ta15 Na5 52.6(3) . . ?
O4 Ta15 O10 88.8(3) . . ?
O4 Ta15 O14 82.0(3) . . ?
O8 Ta15 Na5 119.4(3) . . ?
O8 Ta15 O4 89.8(4) . . ?
O8 Ta15 O10 171.5(3) . . ?
O8 Ta15 O14 86.0(3) . . ?
O10 Ta15 Na5 53.7(3) . . ?
O10 Ta15 O14 85.5(3) . . ?
O14 Ta15 Na5 48.3(2) . . ?
O25 Ta15 Na5 116.4(3) . . ?
O25 Ta15 O4 166.3(4) . . ?
O25 Ta15 O8 90.0(4) . . ?
O25 Ta15 O10 89.4(3) . . ?
O25 Ta15 O14 84.3(3) . . ?
O32 Ta15 Na5 132.5(3) . . ?
O32 Ta15 O4 97.6(4) . . ?
O32 Ta15 O8 92.5(4) . . ?
O32 Ta15 O10 96.0(4) . . ?
O32 Ta15 O14 178.5(4) . . ?
O32 Ta15 O25 96.0(4) . . ?
O3 Ta16 Ta19 42.0(2) . . ?
O3 Ta16 O36 73.3(3) . . ?
O4 Ta16 Ta19 127.5(3) . . ?
O4 Ta16 O3 85.5(3) . . ?
O4 Ta16 O13 92.9(4) . . ?
O4 Ta16 O21 98.8(4) . . ?
O4 Ta16 O27 161.0(4) . . ?
O4 Ta16 O36 86.5(4) . . ?
O4 Ta16 O71 95.7(4) . . ?
O13 Ta16 Ta19 81.4(3) . . ?
O13 Ta16 O3 81.4(3) . . ?
O13 Ta16 O21 82.4(4) . . ?
O13 Ta16 O36 154.7(4) . . ?
O13 Ta16 O71 127.1(4) . . ?
O21 Ta16 Ta19 131.4(3) . . ?
O21 Ta16 O3 163.5(4) . . ?
O21 Ta16 O36 122.7(4) . . ?
O21 Ta16 O71 44.7(4) . . ?
O27 Ta16 Ta19 35.7(3) . . ?
O27 Ta16 O3 77.1(3) . . ?
O27 Ta16 O13 92.0(4) . . ?
O27 Ta16 O21 100.0(4) . . ?
O27 Ta16 O36 81.3(3) . . ?
O27 Ta16 O71 95.8(4) . . ?
O36 Ta16 Ta19 79.1(2) . . ?
O71 Ta16 Ta19 129.0(3) . . ?
O71 Ta16 O3 151.2(4) . . ?
O71 Ta16 O36 78.0(4) . . ?
Ta18 Ta17 Ta19 63.36(2) . . ?
O3 Ta17 Ta18 40.9(2) . . ?
O3 Ta17 Ta19 41.2(2) . . ?
O8 Ta17 Ta18 84.5(2) . . ?
O8 Ta17 Ta19 129.8(2) . . ?
O8 Ta17 O3 89.2(3) . . ?
O8 Ta17 O24 87.4(3) . . ?
O8 Ta17 O36 80.0(3) . . ?
O8 Ta17 O37 100.5(4) . . ?
O8 Ta17 O48 96.6(4) . . ?
O24 Ta17 Ta18 34.2(3) . . ?
O24 Ta17 Ta19 85.8(3) . . ?
O24 Ta17 O3 74.8(3) . . ?
O24 Ta17 O36 145.6(4) . . ?
O36 Ta17 Ta18 112.2(2) . . ?
O36 Ta17 Ta19 78.4(2) . . ?
O36 Ta17 O3 73.2(3) . . ?
O37 Ta17 Ta18 118.7(3) . . ?
O37 Ta17 Ta19 128.1(3) . . ?
O37 Ta17 O3 156.9(4) . . ?
O37 Ta17 O24 84.6(4) . . ?
O37 Ta17 O36 129.0(4) . . ?
O37 Ta17 O48 44.6(4) . . ?
O48 Ta17 Ta18 163.2(3) . . ?
O48 Ta17 Ta19 125.3(3) . . ?
O48 Ta17 O3 155.5(4) . . ?
O48 Ta17 O24 129.0(4) . . ?
O48 Ta17 O36 84.4(4) . . ?
O57 Ta17 Ta18 88.4(3) . . ?
O57 Ta17 Ta19 33.9(3) . . ?
O57 Ta17 O3 75.1(3) . . ?
O57 Ta17 O8 162.5(4) . . ?
O57 Ta17 O24 95.6(4) . . ?
O57 Ta17 O36 88.0(4) . . ?
O57 Ta17 O37 96.9(4) . . ?
O57 Ta17 O48 94.8(4) . . ?
O3 Ta18 Ta17 41.8(2) . . ?
O12 Ta18 Ta17 125.9(3) . . ?
O12 Ta18 O3 84.1(4) . . ?
O12 Ta18 O24 159.9(4) . . ?
O12 Ta18 O29 87.0(4) . . ?
O12 Ta18 O32 92.2(4) . . ?
O12 Ta18 O60 96.8(4) . . ?
O12 Ta18 O89 100.2(4) . . ?
O24 Ta18 Ta17 34.8(3) . . ?
O24 Ta18 O3 76.4(3) . . ?
O24 Ta18 O29 82.8(4) . . ?
O24 Ta18 O32 89.6(4) . . ?
O24 Ta18 O60 98.2(4) . . ?
O24 Ta18 O89 99.9(4) . . ?
O29 Ta18 Ta17 78.7(3) . . ?
O29 Ta18 O3 73.3(3) . . ?
O32 Ta18 Ta17 81.2(2) . . ?
O32 Ta18 O3 81.2(3) . . ?
O32 Ta18 O29 154.5(4) . . ?
O60 Ta18 Ta17 130.0(3) . . ?
O60 Ta18 O3 152.2(4) . . ?
O60 Ta18 O29 79.0(4) . . ?
O60 Ta18 O32 126.3(4) . . ?
O60 Ta18 O89 45.0(4) . . ?
O89 Ta18 Ta17 131.0(3) . . ?
O89 Ta18 O3 162.2(4) . . ?
O89 Ta18 O29 124.0(4) . . ?
O89 Ta18 O32 81.3(4) . . ?
Ta16 Ta19 Ta17 63.865(19) . . ?
O3 Ta19 Ta16 41.2(2) . . ?
O3 Ta19 Ta17 41.3(2) . . ?
O15 Ta19 Ta16 83.5(3) . . ?
O15 Ta19 Ta17 130.8(3) . . ?
O15 Ta19 O3 89.8(4) . . ?
O15 Ta19 O27 87.8(4) . . ?
O15 Ta19 O29 82.0(4) . . ?
O15 Ta19 O49 97.2(4) . . ?
O15 Ta19 O57 162.4(4) . . ?
O15 Ta19 O66 101.4(4) . . ?
O27 Ta19 Ta16 35.0(2) . . ?
O27 Ta19 Ta17 85.2(2) . . ?
O27 Ta19 O3 75.7(3) . . ?
O27 Ta19 O29 146.4(3) . . ?
O29 Ta19 Ta16 111.7(2) . . ?
O29 Ta19 Ta17 77.8(2) . . ?
O29 Ta19 O3 72.4(3) . . ?
O49 Ta19 Ta16 164.2(3) . . ?
O49 Ta19 Ta17 124.3(3) . . ?
O49 Ta19 O3 154.2(4) . . ?
O49 Ta19 O27 129.2(4) . . ?
O49 Ta19 O29 84.0(4) . . ?
O49 Ta19 O57 94.1(4) . . ?
O57 Ta19 Ta16 89.3(3) . . ?
O57 Ta19 Ta17 33.0(3) . . ?
O57 Ta19 O3 74.3(4) . . ?
O57 Ta19 O27 95.5(4) . . ?
O57 Ta19 O29 85.9(4) . . ?
O66 Ta19 Ta16 119.8(3) . . ?
O66 Ta19 Ta17 126.3(3) . . ?
O66 Ta19 O3 157.2(4) . . ?
O66 Ta19 O27 84.9(4) . . ?
O66 Ta19 O29 128.4(4) . . ?
O66 Ta19 O49 44.4(4) . . ?
O66 Ta19 O57 96.2(4) . . ?
O12 Ta20 O15 88.3(4) . . ?
O12 Ta20 O26 174.6(4) . . ?
O12 Ta20 O34 90.5(4) . . ?
O13 Ta20 O12 94.0(4) . . ?
O13 Ta20 O15 88.5(4) . . ?
O13 Ta20 O26 90.8(4) . . ?
O13 Ta20 O34 173.4(4) . . ?
O13 Ta20 O35 96.5(4) . . ?
O15 Ta20 O34 86.8(4) . . ?
O26 Ta20 O15 89.4(4) . . ?
O26 Ta20 O34 84.5(4) . . ?
O35 Ta20 O12 90.6(4) . . ?
O35 Ta20 O15 174.9(4) . . ?
O35 Ta20 O26 91.3(4) . . ?
O35 Ta20 O34 88.2(4) . . ?
Ta22 Ta21 Ta24 64.12(3) . . ?
O16 Ta21 Ta22 41.5(2) . . ?
O16 Ta21 Ta24 41.1(2) . . ?
O34 Ta21 Ta22 83.5(3) . . ?
O34 Ta21 Ta24 131.5(3) . . ?
O34 Ta21 O16 90.7(4) . . ?
O34 Ta21 O70 163.3(4) . . ?
O34 Ta21 O73 83.5(4) . . ?
O34 Ta21 O75 88.7(4) . . ?
O34 Ta21 O97 100.9(5) . . ?
O34 Ta21 O101 99.6(5) . . ?
O70 Ta21 Ta22 87.5(3) . . ?
O70 Ta21 Ta24 32.3(3) . . ?
O70 Ta21 O16 73.3(4) . . ?
O70 Ta21 O73 87.2(4) . . ?
O73 Ta21 Ta22 113.2(3) . . ?
O73 Ta21 Ta24 78.0(3) . . ?
O73 Ta21 O16 73.5(3) . . ?
O75 Ta21 Ta22 34.3(3) . . ?
O75 Ta21 Ta24 83.8(3) . . ?
O75 Ta21 O16 75.0(4) . . ?
O75 Ta21 O70 91.8(4) . . ?
O75 Ta21 O73 147.4(4) . . ?
O97 Ta21 Ta22 163.6(3) . . ?
O97 Ta21 Ta24 120.5(4) . . ?
O97 Ta21 O16 152.6(4) . . ?
O97 Ta21 O70 91.7(5) . . ?
O97 Ta21 O73 83.1(4) . . ?
O97 Ta21 O75 129.5(4) . . ?
O101 Ta21 Ta22 118.7(3) . . ?
O101 Ta21 Ta24 127.0(4) . . ?
O101 Ta21 O16 156.7(4) . . ?
O101 Ta21 O70 97.1(5) . . ?
O101 Ta21 O73 128.1(4) . . ?
O101 Ta21 O75 84.3(4) . . ?
O101 Ta21 O97 45.2(5) . . ?
Ta21 Ta22 K1 156.64(6) . 2_666 ?
O16 Ta22 Ta21 42.1(2) . . ?
O16 Ta22 K1 125.1(3) . 2_666 ?
O16 Ta22 O65 72.3(3) . . ?
O35 Ta22 Ta21 81.9(3) . . ?
O35 Ta22 K1 118.6(3) . 2_666 ?
O35 Ta22 O16 81.8(4) . . ?
O35 Ta22 O46 91.1(4) . . ?
O35 Ta22 O65 154.0(4) . . ?
O35 Ta22 O84 127.7(4) . . ?
O35 Ta22 O98 83.6(4) . . ?
O46 Ta22 Ta21 124.6(3) . . ?
O46 Ta22 K1 49.7(3) . 2_666 ?
O46 Ta22 O16 82.5(4) . . ?
O46 Ta22 O65 84.2(4) . . ?
O65 Ta22 Ta21 79.8(3) . . ?
O65 Ta22 K1 77.0(3) . 2_666 ?
O75 Ta22 Ta21 35.8(3) . . ?
O75 Ta22 K1 140.9(3) . 2_666 ?
O75 Ta22 O16 77.0(4) . . ?
O75 Ta22 O35 94.4(4) . . ?
O75 Ta22 O46 157.8(4) . . ?
O75 Ta22 O65 81.5(4) . . ?
O75 Ta22 O84 99.0(4) . . ?
O75 Ta22 O98 101.8(4) . . ?
O84 Ta22 Ta21 132.3(3) . . ?
O84 Ta22 K1 44.9(3) . 2_666 ?
O84 Ta22 O16 150.5(4) . . ?
O84 Ta22 O46 94.6(4) . . ?
O84 Ta22 O65 78.2(4) . . ?
O84 Ta22 O98 44.3(4) . . ?
O98 Ta22 Ta21 132.9(3) . . ?
O98 Ta22 K1 64.8(3) . 2_666 ?
O98 Ta22 O16 165.2(4) . . ?
O98 Ta22 O46 100.2(4) . . ?
O98 Ta22 O65 122.4(4) . . ?
O16 Ta23 Ta24 41.4(2) . . ?
O16 Ta23 O73 73.4(4) . . ?
O26 Ta23 Ta24 125.0(3) . . ?
O26 Ta23 O16 83.6(4) . . ?
O26 Ta23 O50 157.9(4) . . ?
O26 Ta23 O55 92.0(4) . . ?
O26 Ta23 O67 98.5(4) . . ?
O26 Ta23 O73 85.8(4) . . ?
O26 Ta23 O81 100.2(4) . . ?
O50 Ta23 Ta24 34.3(3) . . ?
O50 Ta23 O16 75.5(4) . . ?
O50 Ta23 O55 91.3(4) . . ?
O50 Ta23 O67 97.1(4) . . ?
O50 Ta23 O73 81.6(4) . . ?
O50 Ta23 O81 101.9(4) . . ?
O55 Ta23 Ta24 81.6(2) . . ?
O55 Ta23 O16 80.0(3) . . ?
O55 Ta23 O73 153.4(4) . . ?
O67 Ta23 Ta24 128.9(3) . . ?
O67 Ta23 O16 153.3(4) . . ?
O67 Ta23 O55 126.3(4) . . ?
O67 Ta23 O73 80.2(4) . . ?
O67 Ta23 O81 44.8(4) . . ?
O73 Ta23 Ta24 78.0(3) . . ?
O81 Ta23 Ta24 132.0(3) . . ?
O81 Ta23 O16 161.3(4) . . ?
O81 Ta23 O55 81.5(4) . . ?
O81 Ta23 O73 125.0(4) . . ?
Ta23 Ta24 Ta21 63.17(2) . . ?
O16 Ta24 Ta21 41.0(2) . . ?
O16 Ta24 Ta23 40.6(2) . . ?
O50 Ta24 Ta21 85.7(3) . . ?
O50 Ta24 Ta23 34.5(3) . . ?
O50 Ta24 O16 74.8(4) . . ?
O50 Ta24 O63 83.8(4) . . ?
O50 Ta24 O65 144.6(4) . . ?
O50 Ta24 O76 130.4(4) . . ?
O63 Ta24 Ta21 127.0(3) . . ?
O63 Ta24 Ta23 80.2(3) . . ?
O63 Ta24 O16 86.2(4) . . ?
O63 Ta24 O65 80.3(4) . . ?
O64 Ta24 Ta21 131.1(3) . . ?
O64 Ta24 Ta23 120.7(3) . . ?
O64 Ta24 O16 159.4(4) . . ?
O64 Ta24 O50 86.3(4) . . ?
O64 Ta24 O63 99.7(4) . . ?
O64 Ta24 O65 127.4(4) . . ?
O64 Ta24 O76 45.1(4) . . ?
O65 Ta24 Ta21 79.2(3) . . ?
O65 Ta24 Ta23 111.1(3) . . ?
O65 Ta24 O16 72.8(4) . . ?
O70 Ta24 Ta21 34.8(3) . . ?
O70 Ta24 Ta23 90.5(3) . . ?
O70 Ta24 O16 75.8(4) . . ?
O70 Ta24 O50 98.1(4) . . ?
O70 Ta24 O63 160.6(4) . . ?
O70 Ta24 O64 99.6(5) . . ?
O70 Ta24 O65 87.4(4) . . ?
O70 Ta24 O76 99.0(5) . . ?
O76 Ta24 Ta21 130.2(4) . . ?
O76 Ta24 Ta23 163.9(4) . . ?
O76 Ta24 O16 154.8(4) . . ?
O76 Ta24 O63 94.2(4) . . ?
O76 Ta24 O65 82.4(4) . . ?
Ta4 K1 Ta22 130.50(9) 2_666 2_666 ?
Ta4 K1 Na6 64.60(9) 2_666 2_666 ?
Ta22 K1 Na6 148.65(12) 2_666 2_666 ?
O46 K1 Ta4 103.24(19) 2_666 2_666 ?
O46 K1 Ta22 30.12(18) 2_666 2_666 ?
O46 K1 Na6 158.8(2) 2_666 2_666 ?
O46 K1 O78 114.1(3) 2_666 2_666 ?
O51 K1 Ta4 98.7(2) . 2_666 ?
O51 K1 Ta22 128.0(2) . 2_666 ?
O51 K1 Na6 37.2(2) . 2_666 ?
O51 K1 O46 157.8(3) . 2_666 ?
O51 K1 O59 129.2(3) . 2_666 ?
O51 K1 O78 83.6(3) . 2_666 ?
O51 K1 O82 68.9(3) . 2_666 ?
O51 K1 O84 98.9(3) . 2_666 ?
O51 K1 O18W 90.4(3) . 2_666 ?
O51 K1 O20W 74.7(3) . 2_666 ?
O51 K1 O33W 90.0(3) . 2_666 ?
O59 K1 Ta4 31.10(19) 2_666 2_666 ?
O59 K1 Ta22 102.2(2) 2_666 2_666 ?
O59 K1 Na6 95.6(2) 2_666 2_666 ?
O59 K1 O46 73.0(3) 2_666 2_666 ?
O59 K1 O78 55.5(3) 2_666 2_666 ?
O59 K1 O20W 80.6(3) 2_666 2_666 ?
O78 K1 Ta4 31.01(19) 2_666 2_666 ?
O78 K1 Ta22 128.8(2) 2_666 2_666 ?
O78 K1 Na6 46.6(2) 2_666 2_666 ?
O82 K1 Ta4 30.2(2) 2_666 2_666 ?
O82 K1 Ta22 154.6(3) 2_666 2_666 ?
O82 K1 Na6 34.7(2) 2_666 2_666 ?
O82 K1 O46 132.6(3) 2_666 2_666 ?
O82 K1 O59 61.3(3) 2_666 2_666 ?
O82 K1 O78 26.4(3) 2_666 2_666 ?
O82 K1 O84 153.0(4) 2_666 2_666 ?
O82 K1 O18W 129.9(4) 2_666 2_666 ?
O82 K1 O20W 71.4(3) 2_666 2_666 ?
O84 K1 Ta4 153.1(2) 2_666 2_666 ?
O84 K1 Ta22 29.3(2) 2_666 2_666 ?
O84 K1 Na6 123.9(2) 2_666 2_666 ?
O84 K1 O46 59.4(3) 2_666 2_666 ?
O84 K1 O59 130.4(3) 2_666 2_666 ?
O84 K1 O78 132.8(3) 2_666 2_666 ?
O84 K1 O18W 72.0(3) 2_666 2_666 ?
O84 K1 O20W 130.3(3) 2_666 2_666 ?
O18W K1 Ta4 128.0(3) 2_666 2_666 ?
O18W K1 Ta22 73.1(2) 2_666 2_666 ?
O18W K1 Na6 122.5(2) 2_666 2_666 ?
O18W K1 O46 78.7(3) 2_666 2_666 ?
O18W K1 O59 113.6(3) 2_666 2_666 ?
O18W K1 O78 155.1(3) 2_666 2_666 ?
O18W K1 O20W 59.1(3) 2_666 2_666 ?
O20W K1 Ta4 74.3(2) 2_666 2_666 ?
O20W K1 Ta22 127.8(2) 2_666 2_666 ?
O20W K1 Na6 80.2(2) 2_666 2_666 ?
O20W K1 O46 114.4(3) 2_666 2_666 ?
O20W K1 O78 96.1(3) 2_666 2_666 ?
O33W K1 Ta4 89.8(3) 2_666 2_666 ?
O33W K1 Ta22 76.5(3) 2_666 2_666 ?
O33W K1 Na6 76.3(3) 2_666 2_666 ?
O33W K1 O46 86.8(3) 2_666 2_666 ?
O33W K1 O59 95.4(4) 2_666 2_666 ?
O33W K1 O78 62.9(4) 2_666 2_666 ?
O33W K1 O82 85.6(4) 2_666 2_666 ?
O33W K1 O84 70.0(4) 2_666 2_666 ?
O33W K1 O18W 141.6(4) 2_666 2_666 ?
O33W K1 O20W 155.7(4) 2_666 2_666 ?
O72 Si1 O59 109.0(5) . . ?
O72 Si1 O74 109.3(5) . . ?
O72 Si1 O79 110.6(6) . . ?
O74 Si1 O59 111.6(5) . . ?
O79 Si1 O59 109.5(5) . . ?
O79 Si1 O74 106.8(5) . . ?
O55 Si2 O46 112.2(5) . . ?
O63 Si2 O46 108.7(5) . . ?
O63 Si2 O55 109.3(5) . . ?
O79 Si2 O46 109.5(5) . . ?
O79 Si2 O55 106.6(5) . . ?
O79 Si2 O63 110.5(6) . . ?
O1W Na1 Na2 42.1(3) . . ?
O1W Na1 O81 70.4(3) . . ?
O1W Na1 O93 77.1(3) . 2_667 ?
O1W Na1 O27W 140.6(6) . 2_667 ?
O2W Na1 Na2 42.7(2) . . ?
O2W Na1 O1W 82.4(4) . . ?
O2W Na1 O81 82.4(3) . . ?
O2W Na1 O93 78.6(3) . 2_667 ?
O2W Na1 O53W 167.5(5) . . ?
O2W Na1 O27W 109.1(6) . 2_667 ?
O81 Na1 Na2 61.0(2) . . ?
O93 Na1 Na2 84.8(3) 2_667 . ?
O93 Na1 O81 144.2(4) 2_667 . ?
O93 Na1 O27W 141.2(6) 2_667 2_667 ?
O53W Na1 Na2 125.6(5) . . ?
O53W Na1 O1W 87.8(5) . . ?
O53W Na1 O81 87.0(5) . . ?
O53W Na1 O93 106.8(6) . 2_667 ?
O53W Na1 O27W 74.0(7) . 2_667 ?
O27W Na1 Na2 127.3(5) 2_667 . ?
O27W Na1 O81 73.9(5) 2_667 . ?
Na3 Na2 Na1 126.8(2) . . ?
O1W Na2 Na1 48.1(3) . . ?
O1W Na2 Na3 126.4(3) . . ?
O1W Na2 O2W 91.6(4) . . ?
O1W Na2 O3W 90.2(4) . . ?
O1W Na2 O67 83.9(4) . . ?
O2W Na2 Na1 46.3(3) . . ?
O2W Na2 Na3 90.9(3) . . ?
O3W Na2 Na1 133.5(3) . . ?
O3W Na2 Na3 92.4(3) . . ?
O3W Na2 O2W 174.4(4) . . ?
O3W Na2 O67 85.7(4) . . ?
O4W Na2 Na1 103.1(3) . . ?
O4W Na2 Na3 41.4(3) . . ?
O4W Na2 O1W 85.1(4) . . ?
O4W Na2 O2W 95.1(4) . . ?
O4W Na2 O3W 90.4(4) . . ?
O4W Na2 O67 168.3(4) . . ?
O5W Na2 Na1 136.6(3) . . ?
O5W Na2 Na3 44.4(3) . . ?
O5W Na2 O1W 170.5(4) . . ?
O5W Na2 O2W 91.0(4) . . ?
O5W Na2 O3W 88.1(4) . . ?
O5W Na2 O4W 85.6(4) . . ?
O5W Na2 O67 105.2(4) . . ?
O67 Na2 Na1 72.2(3) . . ?
O67 Na2 Na3 149.7(3) . . ?
O67 Na2 O2W 89.2(4) . . ?
Na3 Na3 Na2 121.8(3) 2_677 . ?
O4W Na3 Na2 44.0(3) . . ?
O4W Na3 Na3 137.0(4) . 2_677 ?
O4W Na3 O5W 86.9(4) . . ?
O4W Na3 O6W 179.4(5) . 2_677 ?
O4W Na3 O6W 92.1(4) . . ?
O4W Na3 O7W 86.3(4) . . ?
O4W Na3 O88 91.1(4) . 1_565 ?
O5W Na3 Na2 43.1(3) . . ?
O5W Na3 Na3 95.7(3) . 2_677 ?
O5W Na3 O7W 78.8(4) . . ?
O5W Na3 O88 172.3(4) . 1_565 ?
O6W Na3 Na2 135.6(3) 2_677 . ?
O6W Na3 Na2 91.8(3) . . ?
O6W Na3 Na3 43.4(3) 2_677 2_677 ?
O6W Na3 Na3 45.0(3) . 2_677 ?
O6W Na3 O5W 95.5(4) . . ?
O6W Na3 O5W 92.6(4) 2_677 . ?
O6W Na3 O6W 88.3(4) . 2_677 ?
O6W Na3 O7W 174.2(5) . . ?
O6W Na3 O7W 93.2(4) 2_677 . ?
O6W Na3 O88 92.0(4) . 1_565 ?
O6W Na3 O88 89.4(4) 2_677 1_565 ?
O7W Na3 Na2 83.1(3) . . ?
O7W Na3 Na3 136.3(4) . 2_677 ?
O7W Na3 O88 93.6(4) . 1_565 ?
O88 Na3 Na2 134.9(3) 1_565 . ?
O88 Na3 Na3 90.9(3) 1_565 2_677 ?
O8W Na4 Na4 45.3(3) . 2_576 ?
O8W Na4 Na4 44.0(3) 2_576 2_576 ?
O8W Na4 O8W 89.4(4) . 2_576 ?
O8W Na4 O40 88.1(3) 2_576 . ?
O8W Na4 O40 98.8(4) . . ?
O8W Na4 O11W 173.5(4) . . ?
O8W Na4 O11W 90.8(4) 2_576 . ?
O40 Na4 Na4 94.8(3) . 2_576 ?
O11W Na4 Na4 134.4(4) . 2_576 ?
O11W Na4 O40 87.7(3) . . ?
O16W Na4 Na4 87.3(3) . 2_576 ?
O16W Na4 O8W 85.9(4) . 2_576 ?
O16W Na4 O8W 90.3(4) . . ?
O16W Na4 O40 169.1(4) . . ?
O16W Na4 O11W 83.2(4) . . ?
O21W Na4 Na4 135.9(4) . 2_576 ?
O21W Na4 O8W 91.3(4) . . ?
O21W Na4 O8W 171.1(4) . 2_576 ?
O21W Na4 O40 83.0(4) . . ?
O21W Na4 O11W 89.6(4) . . ?
O21W Na4 O16W 102.9(4) . . ?
Ta10 Na5 Ta12 66.16(11) . . ?
Ta10 Na5 Ta13 65.23(10) . . ?
Ta10 Na5 Ta15 122.13(18) . . ?
Ta12 Na5 Ta13 70.25(11) . . ?
Ta15 Na5 Ta12 71.06(12) . . ?
Ta15 Na5 Ta13 64.79(11) . . ?
O4 Na5 Ta10 157.8(3) . . ?
O4 Na5 Ta12 99.9(3) . . ?
O4 Na5 Ta13 94.4(2) . . ?
O4 Na5 Ta15 36.0(2) . . ?
O4 Na5 O10 62.1(3) . . ?
O6 Na5 Ta10 38.1(2) . . ?
O6 Na5 Ta12 96.0(3) . . ?
O6 Na5 Ta13 96.8(3) . . ?
O6 Na5 Ta15 159.9(3) . . ?
O6 Na5 O4 163.0(4) . . ?
O6 Na5 O10 127.8(3) . . ?
O6 Na5 O19 64.0(3) . . ?
O9 Na5 Ta10 36.8(2) . . ?
O9 Na5 Ta12 76.8(2) . . ?
O9 Na5 Ta13 32.7(2) . . ?
O9 Na5 Ta15 97.4(3) . . ?
O9 Na5 O4 125.7(3) . . ?
O9 Na5 O6 64.1(3) . . ?
O9 Na5 O10 64.2(3) . . ?
O9 Na5 O19 64.5(3) . . ?
O10 Na5 Ta10 97.2(2) . . ?
O10 Na5 Ta12 78.8(2) . . ?
O10 Na5 Ta13 32.23(19) . . ?
O10 Na5 Ta15 36.4(2) . . ?
O14 Na5 Ta10 101.5(3) . . ?
O14 Na5 Ta12 36.1(2) . . ?
O14 Na5 Ta13 78.1(2) . . ?
O14 Na5 Ta15 40.9(2) . . ?
O14 Na5 O4 64.0(3) . . ?
O14 Na5 O6 131.1(4) . . ?
O14 Na5 O9 100.8(3) . . ?
O14 Na5 O10 66.1(3) . . ?
O14 Na5 O19 67.5(3) . . ?
O19 Na5 Ta10 38.7(2) . . ?
O19 Na5 Ta12 32.0(2) . . ?
O19 Na5 Ta13 76.5(2) . . ?
O19 Na5 Ta15 102.1(3) . . ?
O19 Na5 O4 131.5(4) . . ?
O19 Na5 O10 99.1(3) . . ?
O14W Na5 Ta10 115.1(3) . . ?
O14W Na5 Ta12 172.3(3) . . ?
O14W Na5 Ta13 117.3(3) . . ?
O14W Na5 Ta15 112.5(3) . . ?
O14W Na5 O4 81.2(4) . . ?
O14W Na5 O6 82.3(4) . . ?
O14W Na5 O9 108.9(4) . . ?
O14W Na5 O10 108.2(4) . . ?
O14W Na5 O14 143.4(4) . . ?
O14W Na5 O19 145.4(4) . . ?
O14W Na5 O26W 81.3(4) . . ?
O26W Na5 Ta10 110.8(3) . . ?
O26W Na5 Ta12 91.2(3) . . ?
O26W Na5 Ta13 161.2(4) . . ?
O26W Na5 Ta15 107.1(3) . . ?
O26W Na5 O4 85.6(4) . . ?
O26W Na5 O6 87.9(4) . . ?
O26W Na5 O9 147.6(4) . . ?
O26W Na5 O10 143.5(4) . . ?
O26W Na5 O14 85.1(4) . . ?
O26W Na5 O19 89.4(4) . . ?
O51 Na6 K1 37.6(2) 2_666 2_666 ?
O51 Na6 O98 114.3(4) 2_666 2_666 ?
O82 Na6 K1 37.0(2) . 2_666 ?
O82 Na6 O51 71.4(3) . 2_666 ?
O82 Na6 O98 113.9(4) . 2_666 ?
O82 Na6 O25W 143.7(4) . . ?
O98 Na6 K1 108.7(3) 2_666 2_666 ?
O22W Na6 K1 87.5(3) . 2_666 ?
O22W Na6 O51 78.1(3) . 2_666 ?
O22W Na6 O82 79.2(4) . . ?
O22W Na6 O98 163.8(4) . 2_666 ?
O22W Na6 O25W 110.3(4) . . ?
O25W Na6 K1 107.0(3) . 2_666 ?
O25W Na6 O51 76.4(3) . 2_666 ?
O25W Na6 O98 65.3(3) . 2_666 ?
Ta5 Na7 Ta10 100.2(2) . . ?
Ta5 Na7 Na5 111.8(2) . . ?
Ta5 Na7 Na10 113.8(3) . . ?
Ta10 Na7 Na5 49.18(12) . . ?
Ta10 Na7 Na10 59.5(2) . . ?
O9 Na7 Ta5 130.6(3) . . ?
O9 Na7 Ta10 31.8(2) . . ?
O9 Na7 Na5 38.2(2) . . ?
O9 Na7 O20 58.8(3) . . ?
O9 Na7 O23 162.7(4) . . ?
O9 Na7 O28 55.2(3) . . ?
O9 Na7 Na10 61.2(3) . . ?
O20 Na7 Ta5 82.6(3) . . ?
O20 Na7 Ta10 31.51(19) . . ?
O20 Na7 Na5 80.1(2) . . ?
O20 Na7 Na10 46.1(3) . . ?
O23 Na7 Ta5 32.2(2) . . ?
O23 Na7 Ta10 132.2(3) . . ?
O23 Na7 Na5 132.2(3) . . ?
O23 Na7 O20 109.8(4) . . ?
O23 Na7 O28 142.1(4) . . ?
O23 Na7 Na10 122.0(4) . . ?
O28 Na7 Ta5 172.3(3) . . ?
O28 Na7 Ta10 84.5(2) . . ?
O28 Na7 Na5 75.9(3) . . ?
O28 Na7 O20 98.7(3) . . ?
O28 Na7 Na10 63.3(3) . . ?
Na10 Na7 Na5 98.9(2) . . ?
O28W Na7 Ta5 98.6(4) . . ?
O28W Na7 Ta10 100.4(3) . . ?
O28W Na7 Na5 139.2(4) . . ?
O28W Na7 O9 101.2(4) . . ?
O28W Na7 O20 77.4(4) . . ?
O28W Na7 O23 87.7(4) . . ?
O28W Na7 O28 74.5(4) . . ?
O28W Na7 Na10 42.2(3) . . ?
Ta12 O1 Ta11 103.7(4) . . ?
Ta12 O1 Ta13 145.4(4) . . ?
Ta12 O1 Ta14 99.0(3) . . ?
Ta13 O1 Ta11 96.5(3) . . ?
Ta13 O1 Ta14 105.8(4) . . ?
Ta14 O1 Ta11 97.6(3) . . ?
Na2 O1W Na1 89.8(4) . . ?
Ta5 O2 Ta9 140.5(5) . . ?
Na2 O2W Na1 91.0(4) . . ?
Ta16 O3 Ta17 105.4(4) . . ?
Ta16 O3 Ta19 96.8(3) . . ?
Ta18 O3 Ta16 146.1(4) . . ?
Ta18 O3 Ta17 97.3(3) . . ?
Ta18 O3 Ta19 105.0(4) . . ?
Ta19 O3 Ta17 97.5(3) . . ?
Ta15 O4 Na5 91.4(3) . . ?
Ta16 O4 Ta15 136.9(5) . . ?
Ta16 O4 Na5 131.1(4) . . ?
Na3 O4W Na2 94.7(4) . . ?
Ta14 O5 Ta13 107.7(4) . . ?
Na2 O5W Na3 92.4(4) . . ?
Ta9 O6 Ta10 139.4(5) . . ?
Ta9 O6 Na5 131.3(4) . . ?
Ta10 O6 Na5 89.0(4) . . ?
Na3 O6W Na3 91.7(4) . 2_677 ?
Ta7 O7 Ta5 135.1(5) . . ?
Ta15 O8 Ta17 131.8(4) . . ?
Na4 O8W Na4 90.6(4) . 2_576 ?
Ta10 O9 Ta13 140.0(5) . . ?
Ta10 O9 Na5 90.3(3) . . ?
Ta10 O9 Na7 100.7(4) . . ?
Ta13 O9 Na5 102.1(4) . . ?
Ta13 O9 Na7 113.5(4) . . ?
Na5 O9 Na7 101.4(4) . . ?
Ta13 O10 Ta15 142.7(4) . . ?
Ta13 O10 Na5 99.9(4) . . ?
Ta15 O10 Na5 89.9(3) . . ?
Ta6 O11 Ta7 105.5(4) . . ?
Ta6 O11 Ta8 97.4(4) . . ?
Ta7 O11 Ta8 98.3(3) . . ?
Ta9 O11 Ta6 143.5(4) . . ?
Ta9 O11 Ta7 97.5(4) . . ?
Ta9 O11 Ta8 106.9(4) . . ?
Ta18 O12 Ta20 140.7(5) . . ?
Ta20 O13 Ta16 140.6(5) . . ?
Ta12 O14 Ta15 136.8(4) . . ?
Ta12 O14 Na5 99.3(4) . . ?
Ta15 O14 Na5 90.8(3) . . ?
Ta19 O15 Ta20 133.8(5) . . ?
Ta21 O16 Ta24 97.9(3) . . ?
Ta22 O16 Ta21 96.4(4) . . ?
Ta22 O16 Ta24 105.9(4) . . ?
Ta23 O16 Ta21 105.1(4) . . ?
Ta23 O16 Ta22 145.3(4) . . ?
Ta23 O16 Ta24 98.0(4) . . ?
Ta11 O17 Ta13 110.5(4) . . ?
Ta11 O17 Na10 106.1(5) . . ?
Ta13 O17 Na10 108.0(5) . . ?
Ta11 O18 Ta10 135.4(5) . . ?
Ta10 O19 Na5 88.1(4) . . ?
Ta12 O19 Ta10 140.4(5) . . ?
Ta12 O19 Na5 101.0(4) . . ?
Ta6 O20 Na7 107.3(4) . . ?
Ta6 O20 Na10 111.6(4) . . ?
Ta10 O20 Ta6 141.3(5) . . ?
Ta10 O20 Na7 93.2(4) . . ?
Ta10 O20 Na10 103.2(4) . . ?
Na10 O20 Na7 82.8(4) . . ?
O71 O21 Ta16 68.2(5) . . ?
Ta2 O22 Ta5 136.1(5) . . ?
Ta4 O23 Na7 118.8(4) . . ?
Ta5 O23 Ta4 141.1(5) . . ?
Ta5 O23 Na7 98.6(4) . . ?
Ta18 O24 Ta17 111.0(4) . . ?
Ta14 O25 Ta15 139.9(5) . . ?
Ta23 O26 Ta20 143.6(5) . . ?
Ta16 O27 Ta19 109.3(4) . . ?
Ta13 O28 Na7 109.4(4) . . ?
O51 O28 Ta13 67.4(5) . . ?
O51 O28 Na7 172.5(7) . . ?
Ta18 O29 Ta19 108.2(4) . . ?
Ta8 O30 Ta10 134.4(5) . . ?
Ta8 O30 Na8 106.9(4) . . ?
Ta10 O30 Na8 118.4(4) . . ?
Ta7 O31 Ta6 107.2(4) . . ?
Ta15 O32 Ta18 138.4(5) . . ?
Ta6 O33 Ta5 142.5(5) . . ?
Ta21 O34 Ta20 135.3(5) . . ?
Ta20 O35 Ta22 140.9(5) . . ?
Ta17 O36 Ta16 107.1(4) . . ?
O48 O37 Ta17 68.4(5) . . ?
Ta8 O38 Ta6 110.9(4) . . ?
Ta7 O39 Ta8 112.5(4) . . ?
Ta14 O40 Na4 120.8(4) . . ?
O58 O40 Ta14 67.8(5) . . ?
O58 O40 Na4 119.7(6) . . ?
Ta3 O41 Ta5 141.3(5) . . ?
Ta12 O42 Ta14 110.3(4) . . ?
Ta11 O43 Ta12 108.6(4) . . ?
Ta14 O44 Ta11 111.8(4) . . ?
O69 O45 Ta12 66.8(5) . . ?
Ta22 O46 K1 100.2(3) . 2_666 ?
Si2 O46 Ta22 126.3(5) . . ?
Si2 O46 K1 118.2(5) . 2_666 ?
Ta9 O47 Ta7 108.5(4) . . ?
O37 O48 Ta17 67.1(5) . . ?
O66 O49 Ta19 66.9(5) . . ?
Ta24 O50 Ta23 111.2(4) . . ?
Ta13 O51 K1 129.4(4) . . ?
Ta13 O51 Na6 122.5(4) . 2_666 ?
Na6 O51 K1 105.3(3) 2_666 . ?
O28 O51 Ta13 67.8(5) . . ?
O28 O51 K1 106.9(6) . . ?
O28 O51 Na6 116.3(6) . 2_666 ?
Ta8 O52 Ta9 106.5(4) . . ?
Ta11 O53 Na11 141.2(5) . . ?
O87 O53 Ta11 67.0(5) . . ?
O87 O53 Na11 127.1(7) . . ?
Ta2 O54 Ta3 107.2(4) . . ?
Si2 O55 Ta23 124.8(5) . . ?
Ta4 O56 Ta2 110.6(4) . . ?
Ta17 O57 Ta19 113.1(5) . . ?
O40 O58 Ta14 67.4(5) . . ?
Ta4 O59 K1 99.0(3) . 2_666 ?
Si1 O59 Ta4 125.7(6) . . ?
Si1 O59 K1 120.0(5) . 2_666 ?
Ta18 O60 Na9 135.9(5) . 2_676 ?
O89 O60 Ta18 67.6(5) . . ?
O89 O60 Na9 118.4(7) . 2_676 ?
Ta1 O61 Ta4 109.1(4) . . ?
Ta1 O62 Ta2 98.0(4) . . ?
Ta3 O62 Ta1 98.1(4) . . ?
Ta3 O62 Ta2 104.6(4) . . ?
Ta3 O62 Ta4 145.0(5) . . ?
Ta4 O62 Ta1 106.3(4) . . ?
Ta4 O62 Ta2 96.6(4) . . ?
Si2 O63 Ta24 120.3(6) . . ?
O76 O64 Ta24 67.6(5) . . ?
Ta24 O65 Ta22 108.5(4) . . ?
O49 O66 Ta19 68.7(5) . . ?
Ta23 O67 Na2 128.1(5) . . ?
O81 O67 Ta23 67.7(5) . . ?
O81 O67 Na2 115.6(7) . . ?
O95 O68 Ta9 68.1(5) . . ?
O45 O69 Ta12 68.3(5) . . ?
Ta24 O70 Ta21 112.9(5) . . ?
O21 O71 Ta16 67.1(5) . . ?
Si1 O72 Ta1 121.3(6) . . ?
Ta21 O73 Ta23 106.4(4) . . ?
Si1 O74 Ta3 124.6(5) . . ?
Ta22 O75 Ta21 109.9(4) . . ?
Ta24 O76 Na11 137.6(6) . 1_655 ?
O64 O76 Ta24 67.3(5) . . ?
O64 O76 Na11 119.4(8) . 1_655 ?
Ta1 O77 Ta2 112.9(5) . . ?
Ta4 O78 K1 86.2(4) . 2_666 ?
O82 O78 Ta4 67.9(6) . . ?
O82 O78 K1 53.3(6) . 2_666 ?
Si2 O79 Si1 153.7(7) . . ?
O88 O80 Ta7 68.8(5) . . ?
Ta23 O81 Na1 139.1(5) . . ?
O67 O81 Ta23 67.5(5) . . ?
O67 O81 Na1 109.7(6) . . ?
Ta4 O82 K1 105.3(4) . 2_666 ?
Ta4 O82 Na6 144.8(5) . . ?
Na6 O82 K1 108.3(4) . 2_666 ?
O78 O82 Ta4 66.5(5) . . ?
O78 O82 K1 100.3(7) . 2_666 ?
O78 O82 Na6 97.2(7) . . ?
Ta6 O83 Na10 109.4(5) . . ?
O91 O83 Ta6 68.2(5) . . ?
O91 O83 Na10 177.0(8) . . ?
Ta22 O84 K1 105.8(4) . 2_666 ?
O98 O84 Ta22 67.9(5) . . ?
O98 O84 K1 104.6(7) . 2_666 ?
O93 O85 Ta3 66.9(5) . . ?
Ta3 O86 Ta1 110.6(5) . . ?
Ta11 O87 Na11 134.7(6) . 2_566 ?
O53 O87 Ta11 68.2(5) . . ?
O53 O87 Na11 115.0(6) . 2_566 ?
Ta7 O88 Na3 120.3(5) . 1_545 ?
O80 O88 Ta7 67.1(5) . . ?
O80 O88 Na3 125.8(7) . 1_545 ?
O60 O89 Ta18 67.4(5) . . ?
O92 O90 Ta8 68.0(5) . . ?
O83 O91 Ta6 67.4(5) . . ?
O90 O92 Ta8 67.1(5) . . ?
Ta3 O93 Na1 127.3(5) . 2_667 ?
O85 O93 Ta3 68.0(5) . . ?
O85 O93 Na1 116.2(7) . 2_667 ?
O96 O94 Ta2 66.9(6) . . ?
O68 O95 Ta9 67.9(5) . . ?
O94 O96 Ta2 68.5(6) . . ?
Ta21 O97 Na9 105.1(5) . . ?
O101 O97 Ta21 67.3(6) . . ?
O101 O97 Na9 71.2(7) . . ?
Ta22 O98 Na6 140.6(5) . 2_666 ?
O84 O98 Ta22 67.9(6) . . ?
O84 O98 Na6 147.9(7) . 2_666 ?
O100 O99 Ta1 67.2(6) . . ?
O99 O100 Ta1 67.7(6) . . ?
Ta21 O101 Na9 108.5(6) . . ?
O97 O101 Ta21 67.5(6) . . ?
O97 O101 Na9 77.8(7) . . ?
O30 Na8 O9W 113.1(7) . 2_567 ?
O60 Na9 O97 86.1(4) 2_676 . ?
O101 Na9 O60 83.0(4) . 2_676 ?
O101 Na9 O97 31.0(3) . . ?
O101 Na9 O21W 121.1(5) . 1_655 ?
O21W Na9 O60 67.6(4) 1_655 2_676 ?
O21W Na9 O97 94.8(5) 1_655 . ?
O32W Na9 O60 79.8(4) 2_676 2_676 ?
O32W Na9 O97 165.8(5) 2_676 . ?
O32W Na9 O101 143.2(6) 2_676 . ?
O32W Na9 O21W 81.5(4) 2_676 1_655 ?
O46W Na9 O60 132.3(7) . 2_676 ?
O46W Na9 O97 83.2(5) . . ?
O46W Na9 O101 108.1(6) . . ?
O46W Na9 O21W 67.2(5) . 1_655 ?
O46W Na9 O32W 107.6(6) . 2_676 ?
O53 Na11 O76 72.7(4) . 1_455 ?
O53 Na11 O87 74.0(4) . 2_566 ?
O53 Na11 O18W 124.2(5) . 1_455 ?
O53 Na11 O44W 156.9(5) . 1_455 ?
O76 Na11 O87 94.9(5) 1_455 2_566 ?
O76 Na11 O18W 75.8(4) 1_455 1_455 ?
O76 Na11 O44W 89.4(5) 1_455 1_455 ?
O87 Na11 O18W 64.2(4) 2_566 1_455 ?
O87 Na11 O44W 123.4(5) 2_566 1_455 ?
O18W Na11 O44W 62.4(4) 1_455 1_455 ?
Na11 O18W K1 153.7(5) 1_655 2_666 ?
Na4 O21W Na9 128.9(5) . 1_455 ?
Ta10 Na10 Na7 57.9(2) . . ?
O17 Na10 Ta10 69.3(3) . . ?
O17 Na10 Na7 90.1(4) . . ?
O17 Na10 O83 151.4(5) . . ?
O20 Na10 Ta10 30.1(2) . . ?
O20 Na10 Na7 51.2(3) . . ?
O20 Na10 O17 99.0(4) . . ?
O20 Na10 O83 55.8(4) . . ?
O83 Na10 Ta10 83.9(3) . . ?
O83 Na10 Na7 83.5(4) . . ?
O28W Na10 Ta10 98.7(5) . . ?
O28W Na10 Na7 42.1(4) . . ?
O28W Na10 O17 116.1(7) . . ?
O28W Na10 O20 81.6(5) . . ?
O28W Na10 O83 76.5(5) . . ?
O28W Na10 O50W 106.8(7) . . ?
O50W Na10 Ta10 134.0(6) . . ?
O50W Na10 Na7 142.8(6) . . ?
O50W Na10 O17 126.7(7) . . ?
O50W Na10 O20 117.7(6) . . ?
O50W Na10 O83 66.4(5) . . ?
Na7 O28W Na10 95.7(5) . . ?

_smtbx_masks_special_details     ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 0.000 0.000 0.000 798.3 247.5 ?
2 0.452 -0.096 0.475 20.3 7.7 ?
3 0.548 0.096 0.525 20.3 10.7 ?

_olex2_submission_special_instructions 'No special instructions were received'
